A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE


 Jeffrey Willis
 1 years ago
 Views:
Transcription
1 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE 2014
2 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIA ZHEN (B.Eng. (Hons)), NUS A THESIS SUBMITTED FOR THE DEGREE OF DOCTOR OF PHILOSOPHY DEPARTMENT OF MECHANICAL ENGINEERING NATIONAL UNIVERSITY OF SINGAPORE 2014
3 DECLARATION I hereby declare that the thesis is my original work and it has been written by me in its entirety. I have duly acknowledged all the sources of information which have been used in the thesis. This thesis has also not been submitted for any degree in any university previously. Mao Jia Zhen 22 Mar 2014
4 Acknowledgement Acknowledgement This thesis is submitted in fulfilment of the requirement for award of the degree of Doctorate of Philosophy. The research has been carried out at the Department of Mechancial Engineering, National University of Singapore, during the period of Augest 2009 to July I am deeply indebted to Professor Tay Tong Earn for giving me the opportunity and supervising this work. Especially during the most challenging period of finalising my thesis, without his allaround support and guidance, this work would have never been accomplished. I would also like to thank A/Prof. Vincent Tan Beng Chye, for his invaluable help. The numerous discussions are important to this work. I am very grateful to Doctor Muhammad Ridha and Doctor Sun Xiu Shan for their advices and help. I am truly thankful to Mr. Chiam Tow Jong, Mr. Low Chee Wah and Mr. Abdul Malik Bin Baba for assisting me in my experiments. Lastly, I would like to deeply thank Ms. Wang Xuan, my daughter Mao Dou Dou, my father Mao Cheng Ming and mother Yang Pei Zhi for their love, support and encouragement throughout my life. You are the reason of this work. i
5 Table of Contents Table of Contents Acknowledgement... i Table of Content... ii Summary vi Nonmenclature... viii List of Figures... xiii List of Tables... xxiii Chapter 1 Introduction and Literature Review Introduction to Textile Structural Composites Review of Mechanical Modeling of Textile Composites Review of Damage Modeling of Textile Composites Failure Criteria Progressive Damage Modeling Techniques Aim of the Study Scope and Outline Chapter 2 Multiscale Modeling Approach Material Property Homogenization Method Periodic Boundary Conditions Effective Material Properties PBC Modeling to a 3D RVE Model MicroMechanical Failure (MMF) Theory Stress Amplification Method Micro Stresses Calculated from Meso Stresses Meso Stresses Calculated from Macro Stresses Fiber Failure Criterion Matrix Failure Criterion Progressive Damage Modeling ii
6 Table of Contents Energebased Continuum Damage Mechanic Model Flow Chart Conclusion Chapter 3 Progressive Failure Analysis of Plain Woven Composites Modeling Strategy Micromechanical Model Mesomechanical Model Geometric Modeling Stress Analysis Progressive Failure Analysis Validation by Experiment Macromechanical Model FE Modeling Simulation Result Validation by Experiment Conclusion Chapter 4 Progressive Failure Analysis of NCF Composites Introduction to NCF composites Nonlinear Mechanical Modeling of NCF composites Modeling of Elastoplasticity for Epoxy Resin Elastoplastic Constitutive Model Parameter Identification Nonlinear Stress Amplification Method Method to Determine Nonlinear Coefficient Implementation of Nonlinear Multiscale Modeling Micromechanical Model Mesomechanical Model Case 0 degree Laminate iii
7 Table of Contents Case Biaxial Laminates Simulation Results Experimental Verfication Macromechanical Model Macroscopic Modeling Simulation Results Experimental Verification Conclusion Chapter 5 Extension to Mechanics of Defects in NCF Composites Introduction to Defects Mechanics of Composite Materials Study the Influence of Defects in NCF composites Linear Analysis on Single Laminate Failure Analysis on Biaxial Laminates Defect Characterization Case [0/90] 2s Laminates Case [±45]2s Laminates Conclusion Chapter 6 Conclusions and Recommendations Conclusions Recommendations for Future Work References Appendix A Plain Woven Composites Study A.1 Mesh Convergency Study for Plain Woven RVE Model A.2 Sensitivity Study for Plain Woven Composites iv
8 Table of Contents Appendix B NCF Composites Study B.1 Mesh Convergency Study for NCF RVE Model B.2 Nonlinear COfficients for MesotoMicro Stress Amplification B.3 Nonlinear COfficients for MacrotoMeso Stress Amplification B.4 Sensitivity Study for NCF Composites Article by the author Mao J Z, Sun X S, Ridha M, Tan V B C, and Tay T E. A modeling approach across length scales for progressive failure analysis of woven composites. Applied Composite Materials, 20: , v
9 Summary Summary Recent advances in textile composites require the development of a holistic modeling tool, which involves more than one length scale. Over the past decades, a large number of modeling techniques, capable of predicting accurately the mechanical performance of composite materials covering wider range of length scales are available. However, there is still a strong demand for a computational approach to implement the mechanical analysis for a macroscopic structure based on the microphysical phenomena. With the rapid development of computer power, it is possible to integrate the available modeling tools into a holistic multiscale framework capable of simulating, designing and analyzing the performance of composite materials. In this thesis, a multiscale modeling approach to model the progressive damage in textile composites has been developed. The hierarchical models of textile composites at three different length scales (micro, meso, and macro) are developed with a novel twoway multiscale coupling technique. In this manner, the multiscale stress analysis is performed and the damage mechanisms can be captured within one finite element. Appropriate failure criteria are carefully selected in the present study. In addition, a continuum damage mechanics (CDM) method is used to model the postfailure behavior of the damaged element. The proposed multiscale method is first applied to predict the material stiffness, tensile strength and damage patterns of a central openhole plain woven laminates. Tensile experiment is conducted to verify the analysis result. Consequently, the progressive vi
10 Summary failure analysis based on a nonlinear multiscale modeling approach is implemented for the noncrimp stitched textile composites considering the material nonlinearity of epoxy resin. The global mechanical analysis of unnotched quasiisotropic laminates has been performed and validated by the experiment. Finally, the proposed progressive failure analysis is extended to the defect mechanics of noncrimp stitched composite laminates. The parametric study based on defect modeling indicates the correlation between the void contents and mechanical properties. The numerical analysis result is validated by the experimental data. vii
11 Nomenclature Nomenclature E Σ C C I M Global strain matrix Global stress matrix Stiffness matrix Effective stiffness matrix Identity matrix Stress amplification matrix Subscript, mm, Microscale, Mesoscale and Macroscale Subscript 1,2,3 Directions of material coordinate system where 1 refers to fiber direction Subscript x, y, z Directions of global coordinate system Subscript m Subscript f Subscript I, II, III ε ε σ σ u x, u y u z Matrix phase Fiber phase Delamination mode I, mode II and mode III Strain vector Global strain vector Stress vector Global stress vector Displacements in three coordinate directions xx, yy, zz, xy, xz, yz Six components of the mechanical strain vector in global coordinates viii
12 Nomenclature 11, 22, 33, 12, 13, 23 Six components of the mechanical strain vector in local material coordinates xx, yy, zz, xy, xz, yz Six components of the mechanical stress vector in global coordinates 11, 22, 33, 12, 13, 23 Six components of the mechanical stress vector in local material coordinates EG, Young s modulus and Shear modulus 0 0 E, G Initial effective Young s modulus and shear modulus * * E, G d ij Residual effective Young s modulus and shear modulus Poisson ratio Material properties degradation factor n s Softening factor V Volume domain S Tensile strength S Compressive strength shear S Shear strength vm von Mises stress I 1 First stress invariant I 2 Second stress invariant G c Fracture toughness Superscript 1,2,3,4,5,6 Six boundary conditions u dummy Displacement defined at the dummy point ix
13 Nomenclature X+, Y+, Z+ X, Y, Z x w Master surfaces on a RVE along three global coordinates Slave surfaces on a RVE along three global coordinates Initial distance between the opposite boundary surfaces on a RVE Critical crack open width when the load falls to zero F s Critical load to initiate a crack D MMF V f Z(x) Damage index from TsaiHa failure theory Fiber volume fraction Fiber yarn crimp height eff Effective stress 0 y Initial yield stress f σ, ε p Yield function g σ n H Subscript e Subscript p Subscript L Subscript G Mσ Plastic potential function Gradient of the plastic potential function Tangent modulus Elasticity Plasticity Local coordinate Global coordinate Nonlinear stress amplification matrix 0 M Dσ P stitch Initial stress amplification matrix Nonlinear coefficient matrix Bridging force on the stitches x
14 Nomenclature P a Peak bridging force stitch Displacement of stitching fiber a Displacement of stitching fiber at peak bridging force h A eff a Thickness of laminate Effective crosssection area of stitching fibers Effective tensile stress on the stitching fibers at peak bridging force t n Normal traction for delamination mode I t s Shear traction for delamination mode II t n Shear traction for delamination mode III G n Energy release rate by the mode I normal traction G s Energy release rate by the mode II shear traction G t Energy release rate by the mode III shear traction V V Void contents UD NCF FE FEM FEA 2D 3D MPDM Unidirectional Noncrimp fabric Finite element Finite element method Finite element analysis Twodimensional Threedimensional Material property degradation method xi
15 Nomenclature CDM CAI MD Continuum damage model Compression after impact Molecular dynamics xii
16 List of Figures List of Figures Figure 1.1 Basic textile architectures...1 Figure 1.2 Types of woven fabrics...4 Figure 1.3 Braid angle in biaxial braided fabric....5 Figure 1.4 Multiaxial multiply stitched noncrimp fabrics....6 Figure 1.5 Discretizedsubcell division from representative cell....9 Figure 1.6 3D voxel representative model for woven composite....9 Figure 1.7a Micromechanical model proposed by Totry et al Figure 1.7b Failure envelop in the multiaxial stress space...13 Figure 1.8 2D geometrical model of fiber yarns in plain woven fabric Figure 1.9 Geometrical model for plain woven composite Figure 1.10 FE modeling scheme of the effect of zpin by distributed nonlinear springs: (a) schematic of a DCB test; (b) section of zpinned composite; (c) FE model for this section with distributed springs Figure 1.11 Illustration of deviations of fiber orientations caused by stitching yarn: (a) Cracks in 45 o ply; (b) Channels in 90 o ply xiii
17 List of Figures Figure 1.12 Scheme of RVE model of NCF composites with different fiber orientations: (a) 0 degree; (b) 45 degree; (c) 90 degree...21 Figure 1.13 Scheme of RVE model of NCF composites with additional stitchines: (a) 0 degree; (b) 45 degree...21 Figure 1.14 Crack modeling within the transverse fiber tow of the plain woven unit cell...38 Figure 2.1 Multiscale damage mechanisms of textile composites Figure 2.2 Multiscale modeling strategy of textile composites...44 Figure 2.3 Periodic structure (a) undeformed shape of RVE (b) deformed shape of RVE...46 Figure 2.4 Illustration of displacement continuity condition...47 Figure 2.5 Material property homogenization for a heterogeneous RVE...50 Figure 2.6 Three pairs of boundary surfaces of a 3D RVE model Figure 2.7 Usage of dummy points for PBC modelling...56 Figure 2.8 Microscopic RVE with (a) square fiber arrangement (b) hexagonal fiber arrangement...60 Figure 2.9 Reference points in microscopic RVE: (a). Matrix of square model; (b). Matrix of hexagonal model; (c). Fiber of square and hexagonal models..61 xiv
18 List of Figures Figure 2.10a Reference point selected in fiber yarn based on meso analysis according to σ Figure 2.10b Reference point selected in fiber yarn based on meso analysis according to σ Figure 2.11 Damage modes for textile composite...67 Figure 2.12 Constitutive behavior for the failed element...70 Figure 2.13 Flowchart of the progressive failure analysis implementation...75 Figure 3.1 Local stress contours in square microscale RVE: (a). Longitudinal axial stress σ 11 under BC1; (b). Transverse axial stress σ 33 under BC3; (c). Longitudinal inplane shear stress τ 13 under BC5; (d). Transverse shear stress τ 23 under BC Figure 3.2 Local stress contours in hexagonal microscale RVE: (a). Longitudinal axial stress σ 11 under BC1; (b). Transverse axial stress σ 33 under BC3; (c). Longitudinal inplane shear stress τ 13 under BC5; (d). Transverse shear stress τ 23 under BC Figure 3.3 Typical stress amplification factors and the corresponding reference points in square RVE...84 Figure 3.4 Typical stress amplification factors and the corresponding reference points in hexagonal RVE...85 Figure 3.5 Fiber yarns in mesoscopic RVE of plain woven composites...86 xv
19 List of Figures Figure 3.6 Cross section micrograph of the plain woven composite laminate...87 Figure 3.7 Geometry of fiber yarn...88 Figure 3.8 Threedimensional Modeling of fiber yarn in ABAQUS...90 Figure 3.9 Mesoscale finite element model: (a) Whole RVE (b) resin pocket (c) fiber yarn...91 Figure 3.10 Local orientations prescribed in fiber yarns...92 Figure 3.11 Reference points in yarn under BC1 based on local stress σ Figure 3.12 Reference points in resin pocket under BC1 based on D MMF Figure 3.13 Reference points in yarn under BC4 based on local stress τ Figure 3.14 Reference points in resin pocket under BC4 based on D MMF Figure 3.15 Reference points in yarn under BC3 based on σ Figure 3.16 Reference points in resin pocket under BC3 based on D MMF Figure 3.17 Reference points in yarn under BC5 based on τ Figure 3.18 Reference points in resin pocket under BC5 based on D MMF Figure 3.19 Matrix damage initiation modes in: (a) fiber yarns (ε xx =0.12%); (b) resin pocket (ε xx =0.15%) xvi
20 List of Figures Figure 3.20 Damage evolution of matrix in: (a) fiber yarns (ε xx =0.3%); (b) resin pocket (ε xx =0.3%) Figure 3.21 Damage patterns at: (a) fiber failure initiation in weft yarns (ε xx =1.08%); (b) first significant load drop in resin pocket (ε xx =1.16%) Figure 3.22 Longitudinal stressstrain relation based on meso failure analysis Figure 3.23 Configuration of the VRTM system Figure 3.24 Experiment setup with extensometer Figure 3.25 Comparison of the stressstrain relations between simulation and experiment Figure 3.26 Failure pattern of tested unnotched specimen Figure 3.27 Macroscale FE model for OHT problem Figure 3.28 Progressive damage patterns predicted from macro failure analysis Figure 3.29 Longitudinal stressstrain relation from Macro FE analysis with CDM modeling Figure 3.30 Untested plain woven OHT specimen Figure 3.31 Comparison of results between FE simulation and Experiment Figure 3.32 Tested plain woven OHT specimen xvii
21 List of Figures Figure 4.1 Uniaxial tensile test results for (a) [0/90] ns NCF laminates; (b) and (c) [ 45] ns NCF laminates Figure 4.2 Tensile test samples for pure epoxy resin Figure 4.3 Tensile Test results for pure epoxy resin samples Figure 4.4 Threedimensional hexagonal microscale RVE model Figure 4.5 Stressstrain curve of micromechanical analysis under longitudinal tension Figure 4.6 Stressstrain curve of micromechanical analysis under transverse tension Figure 4.7 Stressstrain curve of micromechanical analysis under longitudinal shear Figure 4.8 Stressstrain curve of micromechanical analysis under transverse shear Figure 4.9 Floating reference point positions under transverse tension Figure 4.10 Predicted globallocal stress relations from micro analysis under transverse tension Figure 4.11 Parameter identification for NCF mesoscale RVE model Figure 4.12 Top view of biaxial NCF fabric Figure 4.13 Import 3D mesoscale RVE geometry to 3D FE mesh xviii
22 List of Figures Figure 4.14 Local stress distribution in the mesoscale RVE under six periodic loading conditions Figure 4.15 Stressstrain curve of meso analysis under six periodic loading conditions Figure 4.16 Predicted matrix damage onsets within fiber yarns and resin rich zones under six periodic loading conditions Figure 4.17 Layouts of biaxial NCF laminates: (a). [0/90] 2s ; (b). [ 45]2s Figure 4.18 Fiber pull out model [43]: (a) Mode I in DCB model; (b). Mode II in 3 point bending model Figure 4.19 Schematic of the bilinear relationship of the fiber bridging Figure 4.20 Local stress contours σ 11 of [0/90] 2s laminates under longitudinal tension BC1: (a). 0 ply; (b). 90 ply Figure 4.21 Local tress contours σ 11 in [ 45]2s laminates under longitudinal tension BC1: (a). 45 ply; (b). +45 ply Figure 4.22 Predicted progressive damages in [0/90] 2s laminates Figure 4.23 Predicted progressive damages in [ 45]2s laminates Figure 4.24 Longitudinal stressstrain curves from simulation results Figure 4.25 Longitudinal stressstrain curves from simulation results xix
23 List of Figures Figure 4.26 Damage patterns of tested [0/90] 2s NCF specimens Figure 4.27 Longitudinal stressstrain curves from simulation results Figure 4.28 Damage patterns of tested [ 45]2s NCF specimens Figure 4.29 Layout of the quasiisotropic NCF laminates Figure 4.30 Arrangement of the spring element representing the throughthickness stitching Figure 4.31a Predicted damages from macromechanical analysis at applied strain 0.18% Figure 4.31b Predicted damages from macromechanical analysis at applied strain 0.33% Figure 4.31c Predicted damages from macromechanical analysis at applied strain 0.38% Figure 4.31d Predicted damages from macromechanical analysis at applied strain 0.65% Figure 4.31e Predicted damages from macromechanical analysis at applied strain 1.29% Figure 4.32 Predicted stressstrain relation from macromechanical analysis Figure 4.33 Failure modes of tested quasiisotropic NCF specimens: (a) Top view for tested specimens; (b) Top view showing matrix damage; (c) Top view showing fiber fracture; (d) Section view showing delaminations xx
24 List of Figures Figure 4.34 Comparison of results between FE simulation and Experiment Figure 5.1 Multiscale defects observed in NCF composites Figure 5.2 Multiscale defects schematic in NCF composites Figure 5.3 Defect modeling strategy in single NCF laminate Figure 5.4 Defect modeled in the FE model Figure 5.5 Stress contours in single NCF laminate: (a). σ 11 under longitudinal tension; (b). σ 22 under transverse tension; (a). τ 12 under inplane shear Figure 5.6 Predicted inplane stiffness reductions with various void contents Figure 5.7 Defect modeling strategy with fixed void content Figure 5.8 Predicted inplane stiffness reductions with fixed void contents Figure 5.9a Defects observed in [0/90] 2s laminates Figure 5.9b Defects observed in [ 45] 2s laminates Figure 5.10 Defects schematic for biaxial NCF composites: (a) defect in [0/90] 2s laminates; (b) defect in [ 45] 2s laminates Figure 5.11 Defect modeling strategy in [0/90] 2s NCF laminates Figure 5.12 Progressive damages in [0/90] 2s NCF laminates xxi
25 List of Figures Figure 5.13 Predicted stressstrain curve from FE simulation of [0/90] 2s NCF laminates Figure 5.14 Defect modeling strategy in [±45] 2s NCF laminates Figure 5.15 Progressive damages in [±45] 2s NCF laminates at different applied strain levels Figure 5.16 Predicted stressstrain curve from FE simulation of [±45] 2s NCF laminates Figure 5.17 Tensile modulus reduction of [±45] 2s NCF laminates Figure 5.18 Tensile strength reduction of [±45] 2s NCF laminates xxii
26 List of Tables List of Tables Table 2.1 Six periodic boundary conditions applied to RVE model Table 2.2 Material properties used in CDM Table 3.1 Material properties of carbon fibers (T300) Table 3.2 Material properties of matrix (Epoxy EPICOTE 1004) Table 3.3 Predicted effective properties of the fiber yarn Table 3.4 Geometrical paramtes measured from the specimens...89 Table 3.5 Predicted effective properties of mesoscale RVE model...93 Table 3.6 Degradation factors for all damage modes in mesomechanical analysis.101 Table 3.7 Experimental and simulation results for plain woven composites Table 3.8 Degradation factors used for different damage modes in macro analysis 112 Table 3.9 Tensile test results for plain woven composites Table 3.10 Sensitivity study for plain woven composites analysis Table 4.1 Material properties obtained from tensile test for epoxy resin samples..130 Table 4.2 Table for local longitudinal shear modulus H xy fitting to simulation result xxiii
27 List of Tables Table 4.3 Table of nonlinear coefficient D 3 (σ zz ) for meso/micro stress amplification Table 4.4 Measured dimensions of NCF mesoscale RVE model Table 4.5 Predicted effective properties of mesoscale RVE model Table 4.6 Table of nonlinear coefficient D 2 (σ yy ) for macro/meso stress amplification Table 4.7 Parameters for interply cohesive interactions Table 4.8 Predicted longitudinal tensile strength Table 4.9 Experimental results of biaxial laminates Table 4.10 Sensitivity study for NCF composites analysis Table 5.1 Simulation results of [0/90] 2s laminates containing mesoscale defects Table 5.2 Simulation results of [±45] 2s laminates containing mesoscale defects xxiv
28 Chapter 1: Introduction and Literature Review Chapter 1 Introduction and Literature Review By combining two dissimilar materials, composites can provide superior performance with their high mechanical properties and low weight. In the past century, they have been one of the most widely used materials in aerospace, civil, automotive, and marine applications. Meanwhile, products of composite materials also start to popularize in sports and leisure industry in recent years. Among the variety of composites, textile reinforced composite form an essential part of this large family, which is defined as the combination of a resin system and the textile fabrics. The typical textile fabrics comprise of fibers. These fibers are first arranged as fiber bundles. Three basic textile architectures are woven, braided and noncrimp stitched textile as illustrated in Fig Figure 1.1 Basic textile architectures 1
29 Chapter 1: Introduction and Literature Review The textile composites were initially used in automotive and aircraft application in 1960 s, and rapidly developed since 1970 s. They differ from the traditional unidirectional (UD) composites in structure and fabrication. In UD composites, all the fibers align in a prepreg along the same direction. But in the textile composites, fibers are first consolidated into fiber yarns. They are then integrated into various fabrics with the textile process. Textile composites have inherent throughthickness performance achieved by the outofplane reinforcement of the fiber bundles. Besides, they provide greater flexibility in processing options. With the preassemblies of the fiber bundles, the composite fabric is formed, which can range from a single planar sheet to a complex threedimensional net structure. In the costwise, the textile process can reduce the labor cost instead of conventional prepregs. Meanwhile, proper usage of the fiberreinforced textile composites in industry requires a good prediction of their behaviors under different loading conditions. Reliable study and design of the textile composite structures also demand a precise description of the material heterogeneity and textile architectures. The length scales of textile composite are usually defined according to their geometrical and material heterogeneities. The design procedure of composites structures usually includes failure analysis. A typical progressive failure analysis involves a model for damage initiation and propagation. In the first place, the stress or strain analysis is carried out by applying certain loading and boundary condition. According to stress or strain distribution obtained from previous analysis, appropriate failure criteria are used to determine whether the damage occurs. In 2
30 Chapter 1: Introduction and Literature Review progressive damage, the last step of the failure analysis involves a stiffness reduction model to simulate a loss in the loadcarrying capability of the damaged parts. For the study of textile composites, due to the complex textile architectures and material system, the failure analysis needs to capture the damage at different length scales and their influences on the overall performance of the composite structure. 1.1 Introduction to Textile Structural Composites In this section, a general description of three basic textile structural composites: woven, braided and noncrimp stitched are present. Their textile architectures and mechanical features are briefly discussed. Woven fabrics are produced by arranging the fiber yarns in a woven style. Normally, there are two types of fiber yarns, which are perpendicular with each other (weft and warp). There are four basic weave styles (plain, twill, satin and basket) as presented in Fig
31 Chapter 1: Introduction and Literature Review (a) Plain (b) 2/2 Twill (c) 5harness satin (d) Basket Figure 1.2 Types of woven fabrics [1] Woven composites provide superior outofplane performance to the UD composites because of the strong interlocking of the fiber bundles. They are widely used in military and aerospace industries for their high delamination and impact resistance. On the other hand, the interlocking causes the crimp of the fiber yarns, which complicates the modeling for analysis and design. Besides, the crimp regions of woven yarns result in the deterioration of the inplane properties. For instance, woven composites have a lower inplane compressive strength than the other textile composites. 4
32 Chapter 1: Introduction and Literature Review Braided fabric can be regarded as the combination of filament winding and weaving. It is normally integrated as a tubular form over a cylindrical mandrel. Fiber yarns are interwound together in the braided performs. The tubular form is available in biaxial and triaxial architectures. The triaxial braided fabric consists of inserting an axial yarn between the braided yarns in either longitudinal or vertical direction. The angle between the bias axis and the braid axis is called braid angle, usually indicated as θ (see Fig.1.3). Figure 1.3 Braid angle in biaxial braided fabric [2] Similar to woven composites, the braided fabric composites have high impact resistance due to the interwound fiber yarns. It is noted that the application of braided composites should be appropriate to the circumstances. Because the braids are woven on the bias in a tubular form, they can provide efficient core reinforcement. They are commonly used in components of tubular structures that are subjected to torsional loads (eg. driver shaft, antennae, masts, etc.). 5
33 Chapter 1: Introduction and Literature Review Noncrimp fabric (NCF) is also known as multiaxial knitted fabric, which has been integrated by consolidating the fibers in plies by stitching or knitting process [48]. The fiber yarns are first spread and then consolidated together prior to the stitching process. Warpknitting technique is normally used to create the stitched perform. This technique allows the replacement of the fiber yarns with any chosen orientation (see Fig, 1.4). A variety of yarn thickness and width can be selected as long as the knitting needles can go through the plies at the position in between them. Figure 1.4 Multiaxial multiply stitched noncrimp fabrics [9] In recent years, NCF composites have attracted more attentions for their low manufacturing cost. They also provide superior inplane mechanical performance to the other textile structural composites (eg. woven, braided, etc.), resulting from the fact that 6
34 Chapter 1: Introduction and Literature Review the fibers are almost noncrimped. However, the needles penetrating the plies may cause local fiber misalignment, discontinuity, and breakage. Those disturbances may affect the permeability of fabrics and deteriorate the mechanical performance of composite structures. 1.2 Review of Multiscale Modeling of Textile Composites In the past two decades, numerous solutions for structural analysis were developed with the increasing application of textile composite. In this section, modeling approaches for mechanical analysis across different length scales of textile composite are presented. Firstly, modeling techniques for textile composites are briefly introduced from the analytical to the numerical method. Then, the finite element (FE) based modeling at different length scales are discussed respectively. Finally, the existing multiscale modeling approaches are introduced. The limitations of those multiscale methods are also identified. In the beginning, a number of analytical approaches have been developed [1013] to establish the constitutive equation of the textile composite material. They were usually used as analysis codes to predict the overall properties and the mechanical response. The simplest method is based on the rule of mixture and Classical Laminate Theory (CLT). In this method, the composite laminates are treated as homogenized materials. Thus the stress or strain distributions within the textile structure can t be computed accurately in a threedimensional (3D) space. In order to include the descriptions of the textile geometry 7
35 Chapter 1: Introduction and Literature Review and heterogeneous material system, the volume partition approaches were developed [1418]. A discretizedsubcell method was proposed by Tabiei and Jiang [14]. As presented in Fig. 1.5, the representative cell was divided into four subcells. They applied a uniform traction boundary condition to each subcell whereby a volumetric averaging was implemented to calculate the effective stress strain relations of the subcell. The effective properties of the representative cell were obtained by combing the stresses and strains in all subcells. Later, Tabiei and Yi [16] extended this discretizedsubcell method to FE analysis which can provide a more accurate prediction on the effective stiffness of woven composites. In addition, Bogdanovich defined a voxel technique [18] to represent the textile architecture of woven composites in threedimensional (3D) space (see Fig. A1.6). In his method, the representative volume of textile composite was defined as homogeneous, anisotropic solid. The effective elastic properties of the representative volume were determined by the volumetric averaging of the stress and strain fields in the subvoxel volumes. 8
36 Chapter 1: Introduction and Literature Review Fi gure 1.5 Discretizedsubcell division from representative cell [14] Figure 1.6 3D voxel representative model for woven composite [18] Most of the volumepartition approaches above can provide reliable predictions of the effective stiffness. However, geometric simplifications have to be conducted when the 9
37 Chapter 1: Introduction and Literature Review representative volume was divided into several regular subcells. In other word, the textile geometry and material inhomogeneities are exempted in those volumepartition methods. Hence, for the analysis involving more complex conditions such as strain localization and fracture, the modeling technique considering the detailed textile architectures is required. Another limitation of the volumepartition methods is that they were usually specific for one type of the textile composite. For other textile composite types, the methods need to be redeveloped. Thus, a more general and flexible modeling method is required to analyze all types of textile composites. In recent decades, with the rapid development of computer power, numerical modeling tools have been extensively used. FE method can provide effective simulations for the stress and failure analysis of textile composites. It usually uses detailed geometrical and material information to develop a high resolution model of a representative volume element (RVE). By taking the advantage of the finite element method, the modeling approach for performing the analysis at different length scales of textile composite can be developed. Prior to that, the clear definition of length scales is necessary according to the inherent hierarchy of textile composite material [19, 20], 1. Microscale ( ) defines the fibers arranged in the fiber yarn. The microscale model usually consists of the fibers embedded in the matrix. The typical diameter of a fiber is about 510μm. Input data at micro level includes the properties and responses of fiber, matrix and their interface. 10
38 Chapter 1: Introduction and Literature Review 2. Mesoscale (m) defines fiber yarns arranged in the textile architecture and the resinrich zones. It is usually represented by a RVE model. The size of a typical RVE ranges from several millimeters to several centimeters. The properties of the fiber yarns such as the fiber directions and yarn stiffness need to be defined as local data of the mesoscale model. 3. Macroscale (M) defines the textile composite part. In the practical engineering design, it is usually limited to the composite specimen or small panels due to the associated computational cost. Based on the definition of length scales, FE based modeling methods can be individually applied to the mechanical analysis at different length scales. They are presented as micromechanical, mesomechanical, and macromechanical analysis in the following paragraphs, respectively. Computational micromechanical model has been applied in numerous studies of composite materials. The typical micromechanical model consists of the matrix and embedded fiber within a material domain. The fiber distribution is assumed periodic so that a RVE can be used. Micromechanical analysis was initially performed to predict the effective properties of the composite ply by computing stress and strain distributions between fibers and matrix [2125]. Also, the influences of the reinforcement volume fraction and distribution on the deformation of the microscale RVE model can be explored [26]. In addition, FE based micromechanical analysis can be applied to 11
39 Chapter 1: Introduction and Literature Review determine the damage mechanism and failure envelop of composite ply because it can resolve detailed stress and strain fields under multiaxial loading conditions [2729]. For instance, Totry et al. [29] proposed a micromechanical method, where the mechanical response under outofplane shear and transverse compression were emulated (see Fig.1.7a). In this method, constitutive models were used for fiber, matrix and interface in the micromechanical model. Epoxy matrix was assumed as isotropic, elastoplastic material and governed by the MohrCoulomb criterion. A series of virtual tests were presented to reproduce the failure behavior under multiaxial stress states. The failure surface of a UD ply was thus obtained (as shown in Fig.1.7) and showed good agreement with Hashin, Puck and LaRc failure criteria. Figure 1.7 (a) Micromechanical model proposed by Totry et al. [29] 12
40 Chapter 1: Introduction and Literature Review Figure 1.7 (b) Failure envelop in the multiaxial stress space [29] The computational mesoscale modeling is the key step in the multilevel description of textile composites [19, 20]. It usually starts from modeling of the internal geometry of textile reinforcements. The geometric modeling is crucial for a precise computational analysis of textile composites because the overall material properties and stress distributions strongly rely on the fabric architecture. The repeating pattern in a textile fabric can be represented by a RVE which is sufficient to describe the internal geometry of textile reinforcements. The geometric modeling includes generating the fiber yarns with textile structure and the resinrich zone. Unlike the microscopic model, the fibers within a yarn herein are not modeled individually. Instead, the yarn is represented as a homogenous solid volume. Several modeling techniques have been developed for textile 13
41 Chapter 1: Introduction and Literature Review composite considering the yarn crimp [3035]. Peirce [30] proposed a simple geometrical model for plain woven fabric in twodimensional (2D) space, where the yarn path was defined as the combination of straight line and circular arc. The circular shape was used to represent the yarn crosssection. In Peirce s modeling, the radius of curvature of yarn path was equal to the yarn diameter which made sure there was no gap between the interlaced yarns at crossovers. In addition, straight line was deployed to describe the yarn path between the crossovers. The limitation of this model was that the yarn flattening induced during the textile processing was not considered. Later, Peirce used an elliptical yarn crosssection to represent the yarn flattening which improved the accuracy of the geometrical model. Naik et al. [3134] developed a 2D geometrical model for the fiber yarns in plain woven fabric, where a periodic sinusoidal shape function was assumed to describe the yarn path. As presented in Fig.1.8, the interlaced yarns were perfectly in contact at crossovers whereby the yarn crosssection can be described according to the yarn path. Based on this geometrical model, the inplane elastic properties were predicted through FE method and the result was consistent with experiment. Later, Naik and Ganesh [34] successfully predicted the failure of the woven composites under uniaxial static tension based on this model. 14
42 Chapter 1: Introduction and Literature Review Figure 1.8 2D geometrical model of fiber yarns in plain woven fabric [34] Shang and Hoa [35] proposed another geometrical model for woven fabric composite based on microscope observation. In this modeling, an elliptical shape was used to describe the yarn crosssection with a constant area. The thickness and width of yarn was used to represent the crosssection shape. Fig.1.9 presents the central path of the horizontal yarn (along xdirection) and the cross sections of the perpendicular yarns. It can be seen that the central path of the yarn in the plain woven RVE model was defined by combining two crimp functions: the elliptical function for the crossover sections (denoted as T ) and the straight line function for the rectilinear section between the crossover segments (denoted as C ). In this study, the parameters identifying those geometrical functions were obtained from the measurement of actual specimen, which included: (1) yarn thickness t, yarn width w, (2) spacing between the crosssection of parallel yarns, and (3) dimensions of the RVE model. The advantage of this model compared to aforementioned geometric modeling is that the textile geometry was modeled as the final equilibrium configuration of the composite after manufacturing. The geometries of the woven composite were described based on the specimen measurement. 15
43 Chapter 1: Introduction and Literature Review Thus the actual influences of the resin infusion on the internal geometries during manufacturing (such as yarn misalignment and yarn flattening) can be taken into account. Figure 1.9 Geometrical model for plain woven composite [35] In addition to the crimp fabric composite (e.g. woven, braided, etc), the mesoscale modeling techniques for NCF composite have been developed as well. For NCF, the crimp model is not of interest because there is almost no outofplane crimping of fiber yarn. Usually, the mesoscale RVE model of NCF composite consists of composite ply and the stitching system [48, 3640]. The stitching can affect the mechanical performance of the composite in both positive and negative way [4]. The positive effect includes the improvement of the outofplane properties provided by the throughthickness stitches. Many studies have been conducted to explore the influence of stitching on the improvement of the delamination toughness [4145]. The increases of both mode I and mode II toughness of carbonreinforced NCF composites were determined experimentally by means of Double Cantilever Beam (DCB) test and Three Point 16
44 Chapter 1: Introduction and Literature Review Bending test, respectively [41, 42]. As a result, the stitching was found to provide an improvement of up to 15 times in mode I delamination toughness and 4 times in mode II delamination toughness. In addition, Sun et al. [46] proposed a FE modeling scheme to study the influence of stitches on mode I delamination toughness for laminated DCB composite specimens. In this method, the stitch was modeled as a twonode beam element. Virtual crack closure technique (VCCT) was used to determine the strain energy release rate and stress intensity factor at the crack tip. Later, a simpler FE modeling scheme was developed by the same group [43, 44], where mode I and mode II delamination toughness of zpin reinforced composite laminates can be calculated through FE method. The nonlinear spring element was used to represent the throughthickness Zpin whereby the pullout process of the Zpin fiber can be simulated. This new FE modeling scheme is presented in Fig.1.10, which shows the arrangement of the nonlinear springs in a Zpinned DCB composite specimen. The bilinear relation between bridging force and fiber pullout distance was defined for the spring element. This constitutive relation was based on the fiber pullout model proposed by Zhang et al. [47] and Liu et al. [48]. Furthermore, Tasi and Chen [45] applied the nonlinear spring element to the study on the mode I strain energy release rate of noncrimp stitched composite. The effect of stitching fiber stiffness on the mode I strain energy release rate was investigated based on the 3D FE model combined with the crack closure integral method. The numerical study results were consistent with the experimental data. 17
45 Chapter 1: Introduction and Literature Review Figure 1.10 FE modeling scheme of the effect of zpin by distributed nonlinear springs: (a) schematic of a DCB test; (b) section of zpinned composite; (c) FE model for this section with distributed springs [43]. On the other hand, the negative influence of stitching on the mechanical performance of NCF composite has been also investigated [4, 40, 49, 50]. As mentioned in the previous section, the needles penetrating the plies during the textile process may cause local fiber misalignment, discontinuity, and breakage. Lomov et al. [4] conducted an experimental observation of the internal geometry of the carbonreinforced noncrimp fabric. 18
46 Chapter 1: Introduction and Literature Review According to their observations, the deviations of fiber orientations caused by the stitching were found near the stitching sites. As presented in Fig.1.11, the rhomboidal shape deviations in 45 o ply were defined as cracks (Fig.1.11a) while channels (Fig.1.11b) were identified as the deviations formed in 90 o ply. The experimental study in [50] revealed that the permeability of fabrics during the resininfusion was affected by those disturbances, which resulted in resinrich zones in NCF composites. It was further explored that the presence of resinrich zone affected the stress distribution and damage pattern. For the study of textile composite containing those resinrich zones, FE method has been extensively used [36, 5053]. For instance, FE based RVE model for biaxial NCF laminates was developed with accurate description of geometries of resinrich zones [50]. The dimensions of the resinrich zones were obtained based on the specimen measurement. The experimental validation in [53] showed that this FE model can provide more accurate prediction of the composite stiffness than CLT. In addition, the FE simulation revealed that the damage pattern was related with the stress concentrations in the plies at the stitching sites. Later, Mikhaluk et al., [51] extended the geometric modeling method in [50] to the analysis of quasiisotropic NCF laminates (see Fig.1.12). The effective mechanical properties were predicted successfully by taking the resinrich zones into account. The relation between stitching pattern and damages was also revealed through failure analysis. In addition, Zhao et al. [52] developed a 2D FE model to study the failure behavior of [0/90] s NCF composite laminates in longitudinal tension. They assumed a circular crosssection of the yarn with the resinrich zone involved in the FE model. The FE simulation indicated that damage developed within the transverse yarn and resin pocket at early loading stage. After the damage propagated into the longitudinal 19
47 Chapter 1: Introduction and Literature Review yarn, final failure of whole laminates occurred very quickly. Tserpes and Labeas [36] developed another approach for simulating the mechanical performance of NCF composite PI joint structure. In this FE model, the stitches were applied as external reinforcements (see Fig.1.13), whose geometries were obtained from the scanned images of actual specimens. 3D elastic beam elements were used to represent the stitches. However, the resinrich zones were not considered in this modeling method. Figure 1.11 Illustration of deviations of fiber orientations caused by stitching yarn: (a) Cracks in 45 o ply; (b) Channels in 90 o ply [4]. 20
48 Chapter 1: Introduction and Literature Review Figure 1.12 Scheme of RVE model of NCF composites with different fiber orientations: (a) 0 degree; (b) 45 degree; (c) 90 degree [51]. Figure 1.13 Scheme of RVE model of NCF composites with additional stitchines: (a) 0 degree; (b) 45 degree [36]. 21
49 Chapter 1: Introduction and Literature Review A computer aided engineering (CAE) tool for the modeling of different textile composites was proposed by Lomov et al. [19, 20, 5460], called WiseTex. It is capable of modeling the accurate geometry of 2D and 3D woven, braided, and noncrimp stitched fabric. The geometry of the yarn is described based on the input data such as yarn width, yarn thickness, yarn shape, etc. Textile fabric can be modeled in the wake of yarn modeling using the textile information such as weave patterns, yarn count, yarn space, etc. If necessary, data from fiber can be used to evaluate the yarn properties. WiseTex can use fabric and yarn data, obtained from manufacturer or standard test, as a starting point for textile composite modeling. Furthermore, several softwares [57] have been developed integrated with WiseTex by the same group. For example, LamTex is applied to model the textile composite laminates based on the fabric model obtained from WiseTex. FETex can export the solid model to a script file, and then perform FE analysis in ANSYS. MeshTex can be used to generate FE meshes directly from WiseTex solid model. In addition to geometrical model, mechanical analysis on the textile fabric can be implemented by this integral software package. For instance, TexComp has been developed to predict the effective stiffness of a textile composite using MoriTanaka inclusion model [57]. To summarize, the advanced textile structural modeling techniques can provide accurate description of internal geometries of textile fabric at meso level. Based on that, meso RVE model can be generated by combining the fabric architecture and the matrix system. After that, the geometrical model can be converted into finite element meshes whereby 22
50 Chapter 1: Introduction and Literature Review FE analysis can be performed to predict the effective material properties and determine the damages. In the engineering application, the overall mechanical performances of composite parts are of interest [61]. Thus, a computational model at macro level is required in the engineering design of composite components. On the other hand, considering the structural hierarchy of textile composite, the macroscopic mechanical performance can be highly influenced by the geometries and mechanical properties at lower levels. Therefore, it is reasonable to implement computational analysis across different length scales to study the macroscopic behavior of textile composite parts. Generally, there are two families of multiscale modeling techniques: localglobal method and globallocal method. In recent decades, the localglobal multiscale modeling techniques have been developed for analysis of heterogeneous materials such as alloy, porous media, and composite materials. They usually involved the material property homogenization schemes based on the following assumption: the heterogeneous material can be replaced by an equivalent homogenous volume. The simplest method to obtain the effective mechanical properties from the heterogeneous microstructure is the rule of mixture. Besides, some other homogenization methods have been developed based on the empirical formulation [10, 18]. Aforementioned volumepartition techniques were also applied to predict the effective stiffness of composite materials [1418]. In addition, Moulinec and Suquet [62] proposed a numerical technique to investigate the local and global response of composites. Their method can directly apply the digital images of real specimens into the numerical analysis. The images provided the data sampled in a grid of 23
51 Chapter 1: Introduction and Literature Review regular spacing whereby the Fourier transforms were used to obtain the overall mechanical response of the unit cell. This method provided an alternative to the unit cell partition. However, it was limited to the analysis of microstructure with uniform crosssection since the 2D digital image was used for microstructure characterization. In addition, the accuracy of the simulation strongly relied on the resolution and contrast of the images. Geers et al. [63] presented that FE method was preferable to other techniques in the localglobal material property homogenization because it can analyze vast types of heterogeneous materials and provide accurate prediction by considering the detailed microstructures. Michel et al. [64] discussed the application of FE approach to predict the effective properties of composite materials with periodic microstructure. They reported that periodic strain and stress fields were necessary for periodic unit cell to make sure the displacement and traction continuity between neighboring unit cells. Using FE method, the effective stiffness of unit cell can be obtained with prescribed overall stress. This method has been compared with the technique proposed in [62]. As a result, both of them can provide comparable results on the test samples. Another micro FE homogenization method for composite was presented by Carvelli and Taliercio [65]. In this method, regular hexagonal pattern RVE was assumed to represent the fiber arrangement in UD composites. The global constitutive law was described based on the volume average of the stress field on the RVE. Incremental form was obtained so that the nonlinear behavior of composites can be modeled. Later, Carvelli and Poggi [66] extended this method to the analysis of woven fabric composites. Twosteps homogenizations were carried in their model. The mechanical properties of fiber yarn were obtained from the microscopic model in [65], where the yarn were considered as UD fiber reinforced composites with 24
52 Chapter 1: Introduction and Literature Review prescribed fiber volume fraction. Then, the macroscopic response of woven composite laminate can be obtained. This method was validated against to experiment and obtain a good agreement [66]. In addition, Lomov et al. [20] has applied Carvelli s homogenization method [65] in their modeling software WiseTex to predict the effective stiffness of fiber yarn and textile composite laminates. Contrary to the localglobal method, the globallocal modeling starts from the macroscopic analysis. The conventional globallocal method included identifying the region of interest when applying the external loads upon the macroscale model [6769]. These regions can be the crack tips, critical regions with high stresses, or potential region where damages will take place. Then, they will be further analyzed with a refined model. The early attempt of globallocal modeling through FE analysis was made by Whitcomb et al. [67]. In their modeling, the global model with coarser mesh was used as a guide to determine the critical regions. Then the local refinement was carried out for the identified regions. The displacements obtained from the global FE model were considered as the external boundary conditions on the local one. NewtonRaphson iterative method was applied to enforce the displacement continuity between the global and local models. Later, Whitcomb [68] extended this globallocal model to the stress analysis of textile composites. The global model of plain woven composite containing nine subcells in 2D space was used and each subcell with refined mesh was defined as local model. Stress analysis was performed under different loading conditions for global model. Again, the displacements of the global model were applied as boundary conditions on the local model. The multiscale FE simulation indicated that the accurate stress can be predicted 25
53 Chapter 1: Introduction and Literature Review only for the interior cell due to the free edge effect on the other exterior cells. Furthermore, Srirengan et al. [69] applied the globallocal stress analysis in [68] to the 3D problem. In this model, the global FE analysis was performed for 3D plain woven composite with coarser mesh. Homogenized material properties were defined for the global model. The ninesubcell configuration proposed in [68] was converted into 3D space. Considering the free edge effect on the exterior cells, only interior cell was used as local model. Detailed textile geometry was described in the local model whereby the local FE analysis was performed. A short cantilever plate problem was solved to validate the proposed multiscale modeling method. The proposed globallocal model provided a consistent prediction with another FE model using detailed geometry for the entire plate. One of the limitations of the globallocal modeling above is that the detailed local mechanical response can only be studied on the specific region of interest. In addition, because the local analysis performed based on the global phenomenon, when nonlinear constitutive model or damage are taken in account, some parameters are usually required based on empirical model to reproduce the material behavior such as plastic yielding, damage onset and propagations. That requires a large number of reliable data to predict the progressive material responses and the accuracy is problematic if complex loading conditions and environment are involved [70]. To overcome those limitations, Takano et al. [71] has discussed the possibility of modeling a twoway multiscale modeling method where the homogenization method can be used to obtain the global properties from local model while the local stress fields were calculated from global stress to determine the failure mode at local level. However, the direct link between the external loads and the 26
54 Chapter 1: Introduction and Literature Review local stress was not well established in their work. It was also reported that appropriate failure criterion should be developed in the multiscale modeling approach to capture the \ local damage modes. To explore this issue, a literature review of failure approach for textile composites is presented in the next section. 1.3 Review of Damage Modeling of Textile Composites To study the progressive mechanical behavior of the fiberreinforced composite structures, an accurate analysis shall consider the possible damage mechanisms (e.g., tensile fracture of fiber, fracture of matrix, delamination, fiber kinking) and the complex interactions among them. For textile composites, the damage conditions are more complex because of the textile geometry and material inhomogeneities. The textile composite analysis should capture the influences of the textile architectures formed by the fiber yarns on the damage onset and propagation in the ply (meso level), as well as the damage evolution processes within the fiber yarns (micro level). The multiscale nature of damage in textile composites requires damage modeling at different length scales. At each level, appropriate failure criterion and damage modeling technique should be applied. This section discusses the literature of various failure criteria and the progressive damage modeling techniques which can be adapted for failure analysis of textile composites. 27
55 Chapter 1: Introduction and Literature Review Failure Criteria In the study of composite materials, failure criteria were widely used to determine the condition under which the structure fails. The earliest failure criteria include the Maximum Stress Criterion, which is initially proposed for orthotropic material by Jenkins [72] where the failure condition was predicted according to a stress allowable. Later, Waddoups [73] proposed the Maximum Strain criterion where the strain allowable was used. Presently, these two criteria are still widely used to predict the onset of fiber breakage because of their easeofuse. In addition, Hill [74] extended the von Mises yield criterion from isotropic to anisotropic materials. In his method, a polynomial failure criterion was proposed with identical tensile and compressive strength. Hoffman [75] applied Hill s criterion for the composites by considering the distinct tensile and compressive strengths. Tsai [76] also generalized Hill s criterion to fiberreinforced composites where different longitudinal, transverse and shear failure strengths were specified. The approach now is called TasiHill criterion. Later, Tsai and Wu [77] developed a more general failure criterion with a quadratic form. Their criterion assumed that all stress components affected the composite structure failure, but with different weights of contributions. This criterion is extensively used in the engineering design of composite structures due to its accuracy and convenience. To validate those theories, a number of aforementioned failure criteria were deployed through a FE analysis to predict firstply failure in laminated composites [78, 79], which include Maximum Stress criterion, Maximum Strain criterion, TsaiHill s criterion, Hoffman and TsiaWu s criteria. It was indicated that FE code allowed the user to select the desired failure 28
56 Chapter 1: Introduction and Literature Review criterion to predict the initial failure of a ply in laminated composite. It was also concluded all failure criteria perform equivalent failure predictions when inplane loads were applied. But the results were not consistent when the laminates were subjected to transverse load. For instance, TsaiHill and Maximum Strain criterion predict the similar firstfailure ply and failure load but have different prediction results with the other criteria. In addition to the firstply failure prediction, numerous progressive failure approaches have been developed to model the damage propagation in the composite structure in recent years. For instance, Tsai [80, 81] extended the TsaiWu criterion to a progressive failure criterion where the plybyply progressive damage was predicted until the final fracture of composite laminates. This criterion was validated by experiment in [81] and consistent results were obtained. The details of the progressive damage modeling technique applied in [80] will be presented in the next section. Apart from the polynomial criteria for failure prediction at plylevel, Hashin and Rotem [82] proposed a micromechanics based criterion which first specified the failure criterion for different micro failure modes (fiber failure and matrix failure) of UD plies. Hashin [83, 84] later extended his criterion to the 3D failure analysis. Shahid and Chang [85, 86] further developed Hashin s criteria by considering three micro failure modes: matrix failure, fiber breakage and fibermatrix shearout. In addition, Puck and Schurmann [87, 88] developed a phenomenological criterion for micromechanical failure prediction. In this criterion, fiber failure was predicted by a stress or strain allowable and interfiber failure (also known as matrix cracking) was predicted based on the modified Mohr Coulomb theory. Truong et al. [7, 89] applied Puck criterion to determine the transverse 29
57 Chapter 1: Introduction and Literature Review damage of noncrimp stitched composites while Maximum Stress criterion for fiber failure. It is noted that Puck s criterion still uses the stresses at laminar level. Thus, a number of parameters are needed to reproduce the failure behavior according to experimental data because there is no link between the laminar loads and the local stress fields. Gosse [90, 91] proposed a strainbased failure criterion, also known as the Strain Invariant Failure Theory (SIFT), to predict the constituent failure in composite. In this method, strain amplification matrix was proposed to relate arbitrary deformation at laminar level to the strain state at prescribed points within the micro RVE. Thus, the location of damage in the microstructure can be determined based on the micro strain fields. In addition, thermal mechanical deformations can be taken into account in this criterion. Li et al. [92, 93] has applied SIFT to predict the matrixdominated failure in composite structures including Ibeams and Tcleats. Only first strain invariant was used to predict the failure which provided consistent results with experimental data. Tay et al. [9496] have integrated SIFT with their elementfailure method (EFM) to successfully predict the progressive damage in composite laminates based on 3D FE analysis. Later, Ha [97] developed a stressbased failure criterion, which is known as MicroMechanics of Failure (MMF) criterion. In Ha s method, microstructure stress distributions in fiberreinforced composite were obtained using stress amplification factors to directly link arbitrary laminar stresses to the micro stress field. Stress amplification factors were calculated based on the prescribed reference points within the 3D microscale RVE whereby global failure analysis can be performed to determine local damage modes 30
58 Chapter 1: Introduction and Literature Review according to separate failure criteria. In this method, the modified von Mises failure criterion was used to predict the failure initiation of epoxy matrix considering its distinct tensile and compressive strengths. In addition, Maximum Stress criterion was used to predict the onset of fiber breakage. It was noted that linear elastic material properties were assumed for both matrix and fiber in this work. Stress amplification factors were also calculated as constant because of the linear globallocal stress correlations. Sun et al. [98] incorporated a modified MMF criterion and the noniterative elementfailure method (NEFM) to carry out the progressive failure analysis of fiberreinforced composite. Correction coefficients were added to the stress amplification factors in the original MMF criterion to consider the effect of nonlinear behavior when the matrix under tension and the ply subjected to the inplane shear. Corresponding correction coefficients were calculated based on the matrix tensile failure strain and the ply shear failure strain, respectively. Later, Ha [99] integrated the MMF criterion with a progressive damage modeling to perform the failure analysis of laminated composites. This modified MMF criterion is now called TsaiHa criterion. The progressive damage modeling technique applied in this method will be presented in the next section. A comparison between the leading failure criteria has been carried out in the WorldWide Failure Exercise (WWFE). The first WWFE started in 1995 [ ], which performed an extensive evaluation of nineteen failure criteria based on a wide range of experiments. Both strengths and weaknesses of those theories have been identified based on the qualitative assessments. As a result, aforementioned failure criteria developed by Tsai [80, 81] and Puck [88] have been ranked in the group 1, which exhibited top predictive 31
59 Chapter 1: Introduction and Literature Review capabilities and had less than one fundamental weakness. In addition, the aforementioned TsaiHa theory was enrolled in both second [ ] and third WWFE [106] due to its high accuracy and reliability Progressive Damage Modeling Techniques Predicting only damage onset is usually not sufficient in the mechanical analysis of textile composite as the onset of damage occurs typically at a much lower load than the ultimate failure load. Thus, progressive failure analysis is performed to study the influence of accumulative damage on the mechanical performance. Generally, three approaches are commonly applied in the progressive damage modeling of composite: Material Property Degradation Method (MPDM), elementfailure Method and elementpartition method. A brief review of these approaches is given in this section. Then, the FE based MPDM applied for progressive failure analysis of textile composite is discussed in more detail. Finally, the continuum damage method with smeared crack propagation modeling is introduced. MPDM is a practical approach for progressive damage modeling of composite materials. It treats the material with defects as a homogenous material with no defects but with reduced elastic modulus [ ]. In the beginning, the material properties of damaged composites are modified at the plylevel. In this manner, the damage modes of the plies in the composite laminates are usually classified into fiber failure and matrix cracking. A stress analysis of the composite laminate was usually performed to identify the first ply 32
60 Chapter 1: Introduction and Literature Review failure. For the matrix failure, the stiffness of matrix in the damaged ply was reduced at the onset of the first matrix crack. The Young s modulus in the transverse directions E 2, E 3 and the shear modulus G 12, G 13, G 23 of the damaged ply were then reduced with a fraction of the original value. Here, the subscript 1 refer to the longitudinal fiber direction whereas 2 and 3 refer to the transverse directions. On the other hand, the consequence of the fiber failure was the loss of loadcarrying capability in all directions. When the stiffness of the damaged ply is reduced, a new stress distribution of the laminates is presented. Thereafter, the stiffness reduction scheme is iteratively applied to the new stress distribution and predicts the next ply failure. The analysis is stopped when the final fracture of laminates predicted. MPDM can be incorporated with appropriate failure criterion to perform progressive failure analysis. For example, Liu and Tsai [80] have integrated a progressive damage modeling technique into their quadratic failure criterion. In this method, a microcrack mechanism was modeled when the firstply failure was predicted. Corresponding degradation factors were then assigned for different failure modes. It was noted that the microcrack model for matrix failure was only available when failure was caused by a positive strain component. In the case of compressive strain in transverse direction, only longitudinal fiber failure was considered. In addition, the effect of microcracking on the longitudinal compressive strength was modeled, where an exponential compressive strength degradation model was proposed according to the reduction of longitudinal shear modulus. In [80], the authors suggested using 0.15 as matrix degradation factor, 0.01 for fiber degradation, and 0.1 for compressive strength degradation exponent based on empirical data. This criterion successfully described progressive intralaminar failures of composite laminates in 3D space. In addition, Ha [99] 33
61 Chapter 1: Introduction and Literature Review has applied progressive failure approach to his previous proposed failure criterion MMF. In this method, the failure of fiber and matrix was treated separately. On one hand, the damage evolution of matrix was controlled by a degradation function based on the Kuhn Tucker loadingunloading condition. On the other hand, instantaneous degradation was modeled for the fiber failure, which was independent on the matrix failure. It was also noted that linear elastic properties were assumed in this approach, which may reduce the accuracy of the prediction since many types of epoxy resin exhibit nonlinear behaviors. The Elementfailure approach was initially proposed by Beissel [117]. The concept of this approach was to model crack propagation within FE elements. In his approach, the nodal force was released based on a fraction of the stresses contribute to the nodal forces of the element. The fraction depends on the crack length within the element. Because the failed elements were not removed from the mesh, remeshing is not needed. Tay et al. [118] extended Beissel s approach to analyze the damage and delamination in lowvelocity impact of laminated composites. A new Elementfailure method (EFM) was proposed by Tay et al. [118] for progressive damage modeling in composites under quasistatic loading. This approach reduces computational effort since no remeshing and reformulation of the stiffness matrix is required. The Extendedfinite element method (XFEM) is a popularly used elementpartition methods to study the cracking propagation of composite laminates. Belytschko and Black [119] proposed a discontinuous enrichment function which was applied to the finite element to take account of the presence of a crack. The concept of linear elastic fracture 34
62 Chapter 1: Introduction and Literature Review mechanics was used to derive the enrichment functions around the crack tip based on a local partition of element. Moës et al. [120] developed an elementpartition scheme where the crack propagation can be represented without constant remeshing. Later, Sukumar et al. [121] extended the method for threedimensional crack modeling. A modeling method with branching and intersecting of the crack was proposed. Remmers et al. [122] applied the XFEM to the analysis of delamination growth in thin composite laminates. Recently, J. Bienias et al. [123] carried out a damage analysis of composites at the microscale by using XFEM to model the damage of fiber and matrix. XFEM can be also used to represent the material discontinuity in the composite materials. M. Kastner et al. [124] used the XFEM to compute the effective stiffness of textile composites. In this method, XFEM was applied to represent the material interface by modeling weak discontinuities within a finite element. The number of material interfaces was limited to two. For twointerface element, two enrichment functions were used with two vectors of additional degrees of freedom. The elements were subdivided into tetrahedral integration domains under an automated modeling scheme. The material interfaces were localized according to the microscope images of textile composite. The idealized geometry model was used and the predicted effective stiffness agreed well with experimental data. The FE based MPDM is discussed here that has been extensively used to capture the progressive damage in textile composite. This approach usually predicts the damage within an element and makes reduction on the material properties of that element with damage factor. Using FE method, a number of progressive failure analysis have been performed to study the failure initiation and failure development inside the mesoscale 35
63 Chapter 1: Introduction and Literature Review RVE [52, 58, 71, 111, ]. The property degradation in textile composite can be developed based on existing progressive damage model for UD composite. For instance, Takano [71] proposed a FE modeling of progressive damage for woven and knitted fabric composites using MurakamiOhno damage model [126] where the Hoffman criterion was incorporated to predict the damage onset. In this damage modeling, the damage factors were used to perform the stiffness reductions when the occurrence of damage was defected. The damage factor was changed from 0 (initial undamaged state) to 1 (full damaged state). The different failure modes identified by Murakami for a UD composite [126] have been used here to represent the damage mechanisms within the fiber yarn whereas isotropic damage model was used for failure in resin pocket. Later, Zako [113] applied this damage modeling technique to successfully implement the progressive failure analysis of plain woven composite under uniaxial tension, which revealed that the matrix damage initiated at yarn crossover zones and then propagated to the resin pocket. It was also found that the fiber failure in the longitudinal yarn led to the final failure of the RVE model. In addition, material property degradation model can be developed for specific textile composite. For example, Blackketter et al., [127] proposed a stiffness degradation scheme for graphite/epoxy plain woven composites. FE model was used to estimate the influence of damage development on the stiffness reductions. Tension and shear loadings were applied to the model and the simulation results were validated against to experimental data. Based on this degradation model, progressive damages were predicted by Nicoletto and Riva [125] for twillweave laminates under tension. Tang and Whitcomb [111] applied a modified version of Blackketter s degradation model to a progressive failure analysis of woven composites where the degradation factors were 36
64 Chapter 1: Introduction and Literature Review chosen based on a discrete crack modeling of woven composites [128]. In [128], the stress redistribution due to the discrete cracking in the plain woven composite was investigated through FE analysis. As presented in Fig.1.14, the cracks were modeled in the transverse fiber tow (fill tow) and sixboundary conditions were applied to study the stresses in both cracked and uncracked unit cells. Based on that, a complete degradation factors were suggested for graphite/epoxy plain woven composites. The authors suggested using 0.01 as degradation factor for longitudinal tensile modulus, for transverse modulus degradation in either resin pocket or fiber tow, and for shear modulus. In addition, Zhao et al. [52] extended Blacketter s work to progressive damage modeling of [0/90] s NCF laminated composite which exhibited that different damage onset location and different load levels of initial failure and final failure were predicted for different failure criterion combinations. With experimental verification, the authors suggested the failure criterion combination of using Maximum Stress criterion for the yarn and von Mises or DruckerPrager criterion for the resin pocket. The advantage of aforementioned damage modeling methods is that they can provide a direct selective stiffness reduction according to different damage modes. However, Lomov [129] presented that the assumption of volumewide degradation in the modeling approaches above did not necessarily hold in the FE based progressive failure analysis of textile composites. Their experimental study (including Xray inspection and microscope measurement) exhibited that only a few cracks per yarn are identified rather than a formation of multiple cracks in the damaged textile composite. Thus, the authors suggested a single cracklike defect modeling within a finite element. In this method, the 37
65 Chapter 1: Introduction and Literature Review elastic constants of the element were calculated based on Eshelby s inclusion model considering the inhomogeneity contributed by a crack. Figure 1.14 Crack modeling within the transverse fiber tow of the plain woven unit cell [128]. In fact, prior to Lomove s singlecrack model, the crack modeling method have been developed by several researchers. Kachanov [130] first proposed a continuum damage mechanics (CDM) model where the concept of linear elastic fracture mechanics was applied and the energy release rate was used as the internal state variable for crack propagation. In this method, a cracktipplasticity method was developed which showed that when the crack was initiated and started to propagate, the stress will decrease with the crack opening other than fall to zero immediately. This continuum model was applied in FE analysis by Hillerborg et al. [131] where the fracture toughness was defined as 38
66 Chapter 1: Introduction and Literature Review material properties. Allen et al. [132, 133] developed a continuum damage model in the failure analysis of composite laminates. In this method, the damage evolution in the matrix was modeled based on Kachanov s approach. The predicted results agreed well with experiments. Reddy et al. [134] also proposed a gradual stiffness reduction model with the application of finite element method. A stiffness reduction coefficient was used to control the material property degradation process. It was a value between 0 and 1 where 1 refereed to an undamaged element and 0 refereed to the total failure. His results showed that the gradual stiffness reduction model provided more accurate ultimate load than those stiffness reduction schemes which reduced the material properties of damaged element to zero instantaneously [135, 136]. In addition, a smeared crack model was developed by Pinho et al. [137] where a cohesive crack was modeled inside the element. The basic ideal of the smeared crack modeling was the balance between the strain energy released rate and the fracture toughness of material. In this manner, uniform stiffness degradation can be obtained by smearing out the damage over the whole element volume. It was exhibited that the mesh dependency can be eliminated when a characteristic length of the element involved in the energy balance. However, a maximum critical element size was required to avoid that, an element has more elastic energy than the energy dissipated for the crack formation across it before the failure onset. This energyregularized smeared crack model has been applied by Camanho et al. [138] to investigate the inplane size effects in notched carbon/epoxy laminates. Recently, Chen et al. [139] extended the smeared crack model to the study of the thicknessdependency of fiber direction mode I fracture toughness with a linear postfailure softening law. In this method, the fiber 39
67 Chapter 1: Introduction and Literature Review failure in ply was determined by the Maximum Stress criterion and a linear softening law was modeled for the postfailure behavior. 1.4 Aim of the Study In view of the previous studies, there is need to integrate the available modeling tools into a holistic multiscale framework capable of simulating, designing and analyzing the performance of structures made of textile composites. A new multiscale computational modeling is proposed here to study the mechanical behavior of macroscopic structure based on the microstructural phenomenon. In this approach, the constituent failure modes can be captured at different length scales. Another advantage is that the material properties are defined based on the constitutive model at lower length scale. Therefore, this approach can be performed using properties of constituents (such as fiber and matrix) from manufacturer or standard test. There is no need of additional analysis or experiment to define specific macroscopic properties. In addition, this approach is a general framework which can adapt various textile structural composites. 1.5 Scope and Outline A multiscale modeling approach across three length scales is proposed in this thesis to predict damage progression leading to final fracture of textile composites. Here, the 40
68 Chapter 1: Introduction and Literature Review carbon fiber reinforcement within the yarn is described through micro modeling while the mesoscale RVE includes detailed textile architectures of fiber yarns and infused resin pockets, whereby mechanical performance of macroscopic laminated composite upon quasistatic loading can be studied. A novel twoway information transfer method is proposed across different length scales. On one hand, through appropriate homogenization approach, the local inhomogeneous material is replaced by a global homogenous model with equivalent material properties. On the other hand, multiscale stress states are computed to capture the local failure modes. Micromechanisms of constituent damage (fiber and matrix) can be captured using appropriate failure criteria. The treatment of the damage involves the continuum stiffness reduction based on appropriate damage evolution laws. Nonlinear constitutive models, as well as damage, are also taken into account. Finally, the macromechanical analysis can be conducted based on the prescribed data obtained from the analysis at lower length scales, which is computationally inexpensive. The structure of the thesis is outlined as below. In chapter 2, the methodology of the multiscale modeling approach is introduced for the progressive failure analysis of textile composite laminates. Chapter 3 presents the implementation of the proposed method to the failure analysis of plain woven composites. This method is then developed to a nonlinear multiscale modeling approach for the failure analysis of NCF composites in Chapter 4. Chapter 5 extends the method to study the influence of defects contained in the NCF laminated composites. Finally, Chapter 6 presents the conclusion. 41
69 Chapter 2: Multiscale Modeling Approach Chapter 2 Multiscale Modeling Approach In this chapter, a multiscale modeling approach is developed to perform progressive failure analysis of textile composite laminate. In the proposed approach, textile composite material is treated as macroscopically homogeneous but inhomogeneous at meso and micro length scales. The FE method is used to precisely model the material inhomogeneities and stress localizations. Based on the local stress analysis, damage mechanisms at different length scales can be captured. The multiscale damage modes of textile composite are presented in Fig It is demonstrated that the damage of the macroscopic homogenous part in the textile composites can be indicated by the mesoscopic damage in either fiber yarn or resin pocket. The failure in resin pocket is regarded as damage in isotropic epoxy matrix. Meanwhile, the damage mechanisms within the fiber yarn are represented by the failure modes identified for a UD composite [52, 58, 71, 111, ]. Two microscale failure modes are identified here within the yarn: fiber failure and matrix failure. 42
70 Chapter 2: Multiscale Modeling Approach Figure 2.1 Multiscale damage mechanisms of textile composites Based on the definition of length scales in Chapter 1, three FE models are built and analyzed individually. The schematic diagram of the proposed multiscale modeling approach is illustrated by Fig. 2.2 which includes a twoway bridging algorithm. On one hand, the smeared material properties of macroscale model are obtained from the underlying micromechanical and mesomechanical analysis where a localglobal material property homogenization is performed. On the other hand, a globallocal stress dehomogenization is performed which calculates the mesoscopic and microscopic stresses resulting from stressredistribution following damage at the micro level. According to the multiscale stress fields, the multiscale damage modes in Fig 2.1 can be determined. Once the damage onset is determined, a progressive damage modeling 43
71 Chapter 2: Multiscale Modeling Approach technique is applied to update the macroscopic material properties so that the damage evolution in the composite structure can be predicted. Figure 2.2 Multiscale modeling strategy of textile composites In this chapter, we elaborate the proposed multiscale modeling approach from the following aspects. In the beginning, section 2.1 presents the localglobal material property homogenization method with periodic boundary conditions (PBC) imposed on the RVE model. Then, section 2.2 interprets TsaiHa theory which includes the globallocal stress amplification method and the failure criteria for separate constituent failure modes. The smeared continuum damage modeling method is demonstrated in section 2.3 to describe postfailure behavior of damaged element. Finally, the computational 44
72 Chapter 2: Multiscale Modeling Approach implementation of the progressive failure analysis is illustrated by a flow chart in section Material Property Homogenization Method based on Periodic Boundary Conditions Periodic RVE has been widely used to investigate the effective material properties of composites. NematNasser and Hori [140] reported that the predicted effective material properties were dependent on the applied boundary conditions on a RVE. The earlier applied uniform displacement condition (also known as planeremainsplane condition) and uniform traction boundary condition predicted the upper and lower bounds of the effective stiffness, respectively. It was also concluded that the usage of the periodic boundary conditions (PBC) can guarantee more accurate results. Subsequently, Li et al. [141] and Xia et al. [142, 143] proposed a general periodic boundary constraint approach for micro analysis of composites where FE analysis for a micro RVE was performed to predict the effective mechanical properties of composite laminates. PBC was further extended to the analysis of textile composites by Tang and Whitcomb [144, 145]. This systematic approach was derived from the concept of equivalent subcells in [144] where the general equations for subcells were formulated by introducing two vectors: subcell vector and constant vector. The constant vector is a reference vector indicating the direction and distance of the whole cell from the origin whilst subcell vector is added to the constant vector to indicate the absolute position of the subcells. In this section, the general boundary conditions proposed by Xia et al. [142, 143] are presented. They are 45
73 Chapter 2: Multiscale Modeling Approach also deployed in this study to perform stress analysis and predict effective material properties through calculating the average stress and strain tensors of a RVE Periodic Boundary Conditions The periodic array of the RVE is shown in Fig.2.3 where two continuities must be satisfied for the neighboring RVEs. One is displacement continuity at opposite boundaries which guarantees that the neighboring RVEs will neither be separated nor overlapped at the boundaries. The other one is traction continuity which implies the same traction distributions at the opposite boundaries. Figure 2.3 Periodic structure (a) undeformed shape of RVE (b) deformed shape of RVE [143]. For continuous displacements, the displacementdifference boundary conditions are written as [142] 46
74 Chapter 2: Multiscale Modeling Approach j j j j j j i i ik k k ik k i u u x x x c (2.1) As shown in Fig. 2.4, j ui indicate the displacements of node, where i = x, y, and z, represent the directions of nodal displacement. j+ and j denote the jth pair of two opposite boundary surfaces of a RVE. ik is the global strain tensor of the periodic structure. j x k are constants for each pair of the boundary surfaces. Since j x k indicate the initial distances between the opposite parallel boundaries, they are available only when k = j ( j x k = 0 when k j). Here, the constants j ci represent the average deformations of the RVE. When i = j, normal stretch or contraction are applied, whereas the case of i j represents shear deformations. It is noted that, under this displacementdifference boundary condition, the original plane doesn t necessarily remain a plane after the deformation (see Fig. 2.4). In addition, Eq. 2.1 doesn t require the value of displacement at each boundary. Instead, the displacement differences j c i need to be specified between two opposite boundaries. Using FE method, the above displacementdifference functions can be easily used as nodal displacement constraint equations [143]. Figure 2.4 Illustration of displacement continuity condition 47
75 Chapter 2: Multiscale Modeling Approach In addition to displacement continuity, the traction continuity conditions are guaranteed by the equation below [143]: j ik j 0 (2.2) ik Where σ ik are the stresses on the parallel boundary surfaces. When i = k, normal stresses are represented and shear stresses are represented when i k. In [143], a displacementbased FE analysis was conducted. It was demonstrated that Eq. 2.1 in the displacementbased FE analysis can satisfy the traction continuity condition (see Eq. 2.2) automatically. The reason of Eq.2.1 in the displacementbased FE analysis satisfies the traction continuity condition automatically is because the tractions are reaction forces (stresses) resulting from the deformation. In order to explain this statement, a RVE ABCD made up by four subrves is taken as an example in Fig.2.3a. The periodic displacement differences (according to Eq. 2.1) applied on the larger RVE will produce same deformation for each smaller RVE. It can be seen that the tractions at line EO are continuous, which represents right boundary of sub RVE AEOG and left boundary of sub RVE EBHO. Considering the same deformation of these two sub RVES, same traction distribution can be obtained at the left boundaries AG and EO for AEOG and EBHO, respectively. Thus the traction continuity condition at the opposite boundaries AG and EO for subrve AEOG is satisfied. It should be emphasized here that, the traction continuity condition is automatically satisfied only 48
76 Chapter 2: Multiscale Modeling Approach when the displacementbased analysis is performed. For general problems, both equations 2.1 and 2.2 should be applied for a complete PBC definition Effective Material Properties In this section, the effective stiffness matrix of a RVE is calculated. Displacementbased FE analysis is performed to obtain the average stresses and strains. The localglobal material property homogenization is conducted based on the following assumption: material properties of a heterogeneous material can be represented by the effective properties of an equivalent homogenous one (as shown in Fig. 2.5). Thereafter, the average stiffness matrix of a RVE can be used to represent the effective material properties of composite material. The average stresses and strains over a RVE can be written as [143]: 1 ij = ijdv V (2.3) V 1 ij = ijdv V (2.4) V where ij and ij indicate the average stresses and strains, respectively. V denotes the volume of the RVE. 49
77 Chapter 2: Multiscale Modeling Approach Figure 2.5 Material property homogenization for a heterogeneous RVE. The divergence theorem and the equilibrium equation div (σ) = 0 in V and is used to express the volumeaverage stresses as an integration over boundary surfaces [146, 147] 1 1 ij = ijdv = ik x jnkds V V (2.5) V S Where n k indicate the unit vector normal to the boundary surface, which has only one nonzero component (unity value) on each surface. Applying the periodic stress condition (Eq. 2.2), the above equation can be rewritten as [142] 1 1 ij = ( ik x j ds ik x j ds) ik x j x j ds V V j j (2.6) S k S k Sk Recalling that when k j, x x =0. Thus Eq. 2.6 can be expressed as [143] j j 50
78 Chapter 2: Multiscale Modeling Approach x j ij = ijds V S j Pij S j (2.7) Where the average stresses can be calculated from the total tractions on the boundary nodes and the area of the corresponding surfaces, which can be easily obtained from the FE analysis. Meanwhile, the divergence theorem is also used to calculate the volumeaverage strains in the RVE [146, 147] 1 1 j j i i ij = ijdv = (ui ui ) n jds (u j u j ) ni ds V 2V V S j S i (2.8) Applying the periodic strain condition in Eq. 2.1, above equation can be rewritten as [142] 1 2V c S c S j i ij i j j i (2.9) Therefore, the average strains equation can be obtained [142] 1 j ci ij 2 xi i c j x j (2.10) To calculate the effective stiffness matrix of the RVE, the global stressstrain relation of the RVE mode can be expressed as 51
79 Chapter 2: Multiscale Modeling Approach 1 C ΣE (2.11) Σ and E denotes the average stress and strain matrix, respectively. They can be obtained based on Eq. 2.7 and Eq with six boundaryvalue problems. 66 global stress and strain arrays can be obtained to determine the stiffness matrix C PBC of a 3D RVE model In this section, displacement differences equations defined in Eq. 2.1 are applied as nodal displacement constraint equations to a 3D RVE model. Three pairs of opposite boundary surfaces are indentified for a 3D RVE model in Fig. 2.6: 1. X/X+ pair of surfaces normal to x axis 2. Y/Y+ pair of surfaces normal to y axis 3. Z/Z+ pair of surfaces normal to z axis 52
80 Chapter 2: Multiscale Modeling Approach Figure 2.6 Three pairs of boundary surfaces of a 3D RVE model As described in Fig. 2.6, the dimensions of a RVE are defined by L, W and H. The X+, Y+ and Z+ planes are taken as the master surfaces (the nodes on those surface are called master nodes), whereas the opposite X, Y and Z planes are taken as slave surfaces. Every node on the slave surfaces (also known as slave node) corresponds to the node on the master surface (with the same inplane coordinates). In the proposed constraint equation, displacements of the slave nodes should coincide with the displacements of corresponding master nodes so Eq. 2.1 can be rewritten as u u c (2.12) j j j i, slave i, master i j j In the equation above, ui, slave and u, i master denote the displacements of the slave node and its corresponding master node, respectively. i = x, y and z, indicates the normal direction to three pairs of boundary surfaces, and j = x, y, and z, represents three directions of nodal 53
81 Chapter 2: Multiscale Modeling Approach displacement. For each pair of boundary surface, the displacement differences j ci are used to represent the deformations of the RVE. Table 2.1 outlines the six periodic boundary conditions applied to the RVE model (known as BC1 through BC6) where prescribed displacement differences j c i are defined. Using the values of j ci given in Table 2.1, the global strain array E can be calculated according to Eq Meanwhile, the global stress array Σ is acquired from FE simulations under the six boundary conditions (see Eq. 2.7). In the end, the effective stiffness matrix C can be determined according to Eq Table 2.1 Six periodic boundary conditions applied to RVE model 54
82 Chapter 2: Multiscale Modeling Approach When applying the PBCs into the 3D RVE model, three additional dummy points are deployed here corresponding to three pairs of boundary surfaces. Dummy points are the nodes artificially created outside the FE mesh. The displacements of dummy points are related with the displacements of real nodes on the mesh. The prescribed displacement differences defined in Table 2.1 are replaced by the displacements of the dummy point. Hence, Eq, 2.12 can be rewritten as u u c u u (2.13) j j j j j i, slave i, master i i, master i, dummy j Where u, i dummy denotes the displacements of the dummy points. i = x, y and z, indicate three dummy points which govern the relative displacements between ith pair of boundary surfaces. j = x, y, and z, represent the dummy point displacements along three principle axes. Two examples are presented in Fig. 2.7 to illustrate the usage of the dummy points in a 2D plane problem. In Fig. 2.7a, displacement is defined to one of the dummy points along xaxis that represents the displacement differences between all the slave nodes (at left boundary) and their corresponding master nodes (at right boundary) in the xdirection. As a result, a horizontal stretch is created on the RVE with a periodic boundary condition. It is noted that the PBC defined here only constraints the difference of nodal displacement between slave and master node. The left and right boundaries do not necessarily remain straight but they should have the identical deformed profile (as seen in Fig. 2.4). Likewise, an inplane shear deformation is represented by another x dummy point displacement, u, y dummy, which indicates the displacement difference between 55
83 Chapter 2: Multiscale Modeling Approach the slave nodes (at lower boundary) and the corresponding master nodes (at upper boundary) along xaxis. Figure 2.7 Usage of dummy points for PBC modelling To implement those periodic boundary conditions in the FE analysis software  ABAQUS, the command *Equation is used to describe the constraint equations in Eq, The equations of multipoint constraint are written into the ABAQUS input file. In this manner, the nodal displacement differences between the three pairs of opposite surfaces (X/X+, Y/Y+, Z/Z+) are individually modeled. In addition one fixed node needs to be 56
84 Chapter 2: Multiscale Modeling Approach defined on the RVE to avoid the rigid body motion. Most of the time, the node in the center of the RVE is selected for this boundary condition. 2.2 MicroMechanics of Failure (MMF) Theory This section presents the principle of the MicroMechanics of Failure (MMF) theory (also known as TsaiHa theory), which are employed for the first time to predict the damage in textile composite. The MMF theory was proposed by Ha et al. [97] where local stress distributions in fiberreinforced composite can be obtained by linking arbitrary global stress to the local stress field. MMF theory is preferable in this study because it can explicitly distinguish between the different constituent failure modes. Based on that, corresponding failure criteria for the constituent (fiber and matrix) can be applied independently. In addition, this stressbased micromechanics approach allows using the constituent strength values directly from the manufacturer, material handbook, or standard tests to determine the local damage mechanisms. Here, a stress amplification method is introduced to calculate the local stress fields from the global stresses. Then, a set of constituent failure criteria is adopted to determine the damage onset in textile composite Stress Amplification Method To obtain the local stress states, a globaltolocal stress transfer can be performed through the amplification equations below [9799]: 57
85 Chapter 2: Multiscale Modeling Approach σ M σ L G A ΔT (2.14) Where σ L and σ G indicate local and global stress states, respectively. σ G is the external stresses applied upon the RVE while σ L represents the local stress field within the local structure. In addition, ΔT is the temperature increment; M, and A represent the stress amplification factors for global stress and the temperature increment which may vary with positions. FE analysis is performed to determine the stress amplification factors of RVE model. The proposed multiscale modeling approach involves two steps of stress amplification (mesotomicro and macrotomeso), through FE analysis of two RVEs (microscopic and mesoscopic). They are presented separately in following paragraphs Micro Stresses Calculated from Meso Stresses To calculate the micro stress field, the stress amplification equation in Eq can be modified to σ M σ A ΔT m m m m (2.15) Where subscripts and m denote microscale and mesoscale, respectively; M μm and A m indicate the mechanical stress amplification factors and thermal stress amplification factors from meso level to micro level. Prior to the failure analysis, FE analysis is 58
86 Chapter 2: Multiscale Modeling Approach performed to calculate the stress amplification factors with the selected reference points in the microscopic RVE model. Here, two types of micro RVE are used to represent different fiber arrangements: square and hexagonal (see Fig. 2.8a and Fig. 2.8b). To calculate the mesomicro stress amplification factors, reference points are separately selected at the critical regions in the fiber and matrix phase. The critical regions usually represent the locations with high stress concentrations and where damage may occur. Sun et al. [98] chose the reference point locations within a micro RVEs as illustrated in Fig It shows that points 1 through 13 are defined at the fibermatrix interface in both square and hexagonal RVEs (see Fig. 2.9c). In Fig. 2.9a, points 14 through 18 are chosen in the matrix region in the square model. Points 14 through 19 in the matrix of hexagonal were defined in Fig. 2.9b. For each point, a 6 6 stress amplification matrix can be computed by the equation below 1 m M Σ Σ (2.16) μm μ Where μ 1 μ 2 μ 3 μ 4 μ 5 μ 6 μ 6x6 Σ σ σ σ σ σ σ (2.17) m 1 m 2 m 3 m 4 m 5 m 6 m 6x6 Σ σ σ σ σ σ σ (2.18) 59
87 Chapter 2: Multiscale Modeling Approach In the equations above, i σ is the stress array corresponding to different boundary conditions. i = 1 to 6 denote the six boundary conditions applied on the microscopic model. It is noted that the stress amplification factors only need to be calculated once for a given material system. After that, they can be readily applied in the failure analysis. Figure 2.8 Microscopic RVE with (a) square fiber arrangement (b) hexagonal fiber arrangement. 60
88 Chapter 2: Multiscale Modeling Approach Figure 2.9 Reference points in microscopic RVE: (a). Matrix of square model; (b). Matrix of hexagonal model; (c). Fiber of square and hexagonal models [98] Meso Stresses Calculated from Macro Stresses In this study, the MMF theory is extended to the failure analysis of textile composite. FE analysis is performed for the mesoscale RVE model to capture the damage mechanisms at meso constituent level (yarn and resin pocket) arising from the nonuniform meso stresses. To calculate the meso stress field, the stress amplification equation in Eq can be expressed as σ M σ A ΔT m mm M mm M (2.19) Where subscripts m and M denote mesoscale and macroscale, respectively; M mm and A mm indicate the mechanical stress amplification factors and thermal stress amplification 61
89 Chapter 2: Multiscale Modeling Approach factors from macro level to meso level. The macromeso stress amplification factors are computed based on the equation below, 1 M M Σ Σ (2.20) mm m And, M 1 M 2 M 3 M 4 M 5 M 6 M 6x6 Σ σ σ σ σ σ σ (2.21) i σm indicate the macroscopic external stresses applied on the mesoscale model, where i = 1 to 6 denote the six boundary conditions. For Σ M, the mesoscopic stress array i σm described by Eq is regarded as local stress fields here. They are extracted according to the selected reference points within the mesoscale RVE model. The typical reference points identified are presented in Fig when the meso RVE is under a uniaxial tension along xaxis. The reference points within the fiber yarn and resin pocket are chosen separately and the arrangement of the reference points closely follows the local stress distributions on the meso RVE model. As presented in Fig. 2.10a, local longitudinal stress σ 11 (parallel to the fiber direction) is used for identifying the reference points within the fiber yarns. An index D MMF is used for identifying the reference points in the resin pocket (see Fig. 2.10b). D MMF is obtained based on a modified von Mises failure criterion proposed in TsaiHa theory as matrix failure criterion. This criterion will be elaborated later in section
90 Chapter 2: Multiscale Modeling Approach Figure 2.10a Reference point selected in fiber yarn based on meso analysis according to σ 11. Figure 2.10b Reference point selected in epoxy pocket based on meso analysis according to D MMF. 63
91 Chapter 2: Multiscale Modeling Approach The reference points adopted in this method should be able to represent the critical regions in the mesoscale RVE under different external loads. Thus, six boundary problems described in Table 2.1 are solved in the mesoscale stress analysis to obtain a complete set of stress amplification factors. The details of reference point identification and calculation of stress amplification factors will be explained in the mesomechanical analysis of woven (Chapter 3) and NCF composites (Chapter 4), respectively Fiber Failure Criterion In HaTsia theory [99], Maximum Stress criterion is applied to capture the fiber failure initiation. The Maximum Stress criterion is initially proposed by Jenkins [72] from the assumption that failure takes place whenever any one of the stress components attains its critical value. The critical values are determined through a series of tests in which the specimen is under a uniform, uniaxial state of stress. The original form of this criterion is: S S ; S S ; S S S ; S ; S (2.22) Where the superscripts + and  denote the tension and compression, respectively; S 1 indicates the ultimate normal stress in the fiber direction, S 2 and S 3 the ultimate stresses in the two transverse directions, and S 12, S 23 and S 31 the ultimate shear stresses. 64
92 Chapter 2: Multiscale Modeling Approach Ha proposed an alternative for fiber failure prediction using a quadratic failure criterion, which can be written as [99] S S 1 ij i j i i j1 i1 i1 (2.23) The criterion above takes the orthotropy of carbon fiber into account. However, except the longitudinal tensile and compressive strength, there is usually lack of reliable measurements of the other strength values. Thus the above equation can be simplified into a more practical form [99], S S (2.24) Matrix Failure Criterion In Ha s theory, the von Mises failure condition is modified by taking into account the difference between tensile strength S + and compressive strength S . The damage factor D MMF was proposed in [97] to determine the failure initiation of matrix: DMMF 2 vm 1 1 I1 1 S S S S (2.25) Where vm represents the von Mises stress 65
93 Chapter 2: Multiscale Modeling Approach 2 vm I1 3I2 (2.26) and I 1 and I 2 denotes the first and second stress invariant, respectively I I τ τ τ (2.27) In this manner, the damage at matrix and fiber can be predicted separately. Therefore, specific material property degradation factors can be applied corresponding to the different damage mechanisms identified by the failure criteria above. The details of the damage modeling method will be discussed in the next section. 2.3 Progressive Damage Modeling In this section, a progressive damage model is developed, which is incorporated with the Material Properties Degradation Method (MPDM) to describe a postfailure softening behavior of damaged element. It is noted that failure analysis in textile composites involves different damage modes that leads to different influences on the overall effective behavior of composites structures. The damage modes identified in textile composite is presented in Fig [71]. This figure illustrates that the damages within the fiber yarn and in the resin pocket can be distinguished from the damage in the macroscopic textile composite structures. In addition, the damage mechanisms for a UD composite are used to represent the failure modes in the fiber yarn [52, 58, 71, 111, ] where the loss 66
94 Chapter 2: Multiscale Modeling Approach of load carrying capacity in the longitudinal direction is usually attributed to the fiber failure while the reduction of normal transverse properties and shear modulus are mainly governed by the matrix damage. Figure 2.11 Damage modes for textile composite [71] Material properties degradation method is deployed here based on the assumption that a material with damage can be modified by reducing the elastic stiffness. For a failed element, the elastic constants are reduced as below: 67
95 Chapter 2: Multiscale Modeling Approach E d E i j, (2.28) * 0 ij ji ij, G d G i j. (2.29) * 0 ij ji ij, Where and * E ij and * G ij are effective residual material properties of failed element while 0 G ij are the values of initial stiffness. The value of stiffness degradation factor d is given between 0 and 1. The initial value of d is 1, which represents the undamaged state. For different damage modes, corresponding degradation factor is defined as follows, 0 E ij 1. L ongitudinal failure due to fiber fracture: values of d 11, d 22, d 33, d 12, d 13, and d 23 are reduced. 2. Other failure modes due to matrix damage (includes micro matrix damage within the yarn and damage in the resin pocket): values of d 22, d 33, d 12, d 13, and d 23 are reduced, d 11 remains 1. Note that the amounts of stiffness reductions are not constant for all textile composite types. Different degradation scenarios for different textile composites will be discussed separately in the following chapters. 68
96 Chapter 2: Multiscale Modeling Approach Energy Based Continuum Damage Mechanics Model A number of numerical and experimental studies proved that the damages in composite structure exhibited a gradual propagation of fracture [131, ]. In addition, in the proposed multiscale modeling, it is too conservative to remove all the loadcarrying capability from the material of macroscopic structure when the damage occurs in the microstructure. The continuum damage mechanics (CDM) model has been developed via FE method to allow a gradual stiffness reduction within a damaged element [ , ]. In this section, an energy based CDM model proposed by Pinho [137] is deployed to model the crack propagation within a failed element, where the stiffness is degraded, not instantaneously with a constant ratio but gradually according to the current stress state. The basic idea of this smeared crack modeling is the balance between the strain energy released rate and the fracture toughness of material. Considering the energy absorbed by a completely failed element, U, is [137] 0 f U= V (2.30) 2 0 f Where V is the element volume; and indicate the material strength and maximum strain, respectively. Dividing both sides of Eq by the crack surface area, we can obtain [137] 0 f U Le Gc (2.31) A 2 69
97 Chapter 2: Multiscale Modeling Approach Where G c is the fracture energy, which can be determined as the material properties of the material and L e is one element dimension. Thus the constitutive behavior of failed element can be obtained. As illustrated in Fig. 2.12, the reduction of the stiffness is defined by the slope of the softening process, where 0 is the critical stress for crack initiation. Fracture energy G c and characteristic element length L e are used to determine the maximum fracture strain f by Eq. 2.32, f 2Gc 0 L (2.32) e Note that, the critical energy regarded as a material property here, is independent on the element size. Equation 2.32 is developed to ensure this independency, by including the strain to failure and characteristic element. In this manner, even the element size varies, the critical energy value remains constant. Figure 2.12 Constitutive behavior for the failed element [137] 70
98 Chapter 2: Multiscale Modeling Approach Based on the linear softening law described in Fig. 2.12, the softening factor n s is used to represent the ratio between the softened stiffness and initial stiffness [137], min 0, max,1 ( ) f 0 ( ) n s f 0 (2.33) Therefore, the gradual stiffness reduction scheme can be developed by adding the softening factor to the Eq.2.28 and 2.29, * 0 Eij 1 1 ns 1 d ij Eij, i j, (2.34) * 0 Gij 1 1 ns 1 d ij Gij, i j (2.35) The softening law is applied for both fiber and matrix failure. The fiber fracture is modeled as Mode I and only the Mode I fracture toughness G fic is used. At the same time, the matrix fracture is modeled as mixmode, and the fracture energy G mc is determined according to the BenzeggahKenane criterion [152]. G G G G ms mc mic miic mic Gmn Gms G m (2.36) Where the superscript m is a semiempirical criterion exponents at different mode ratios. G mn and G ms are fracture energy defined at the damage onset as, 71
99 Chapter 2: Multiscale Modeling Approach G G mn ms l e (2.37) 2 le (2.38) 2 The material properties used in proposed CDM model are listed in Table 2.2. Value of G fic is obtained from the experimental investigation in [153]. Chen et al. [139] used the same value for their thickness dependency study of mode I fracture toughness on multiply laminated composites. The fracture properties for epoxy resin are determined by fitting to experimental data [154]. They were also used in the numerical study of size effect on the tensile strength of composite laminates containing circular central holes [155]. Properties Table 2.2 Material properties used in CDM Values G fic (kj/m 2 ) G mic (kj/m 2 ) 0.2 G miic (kj/m 2 ) 1 m 1 72
100 Chapter 2: Multiscale Modeling Approach 2.4 Flow Chart The flowchart in Fig illustrates the computational implementation of the progressive failure analysis. The algorithm of the present analysis includes the stress amplification, failure prediction, and material degradation process. It comprises of following steps: 1. The FE analysis at macro level is performed with prescribed displacement. The effective material properties predicted through the micro and meso analysis are used as input data. The stress amplification factors are also prepared prior to the macro analysis. 2. Obtain the macroscopic stress by assembling the global stiffness matrix and solving the macroscopic nodal displacements. 3. Perform macrotomeso stress amplification (see Eq. 2.19). Two sets of stress amplification factors are used to calculate the stresses in the fiber yarns and the resin pockets separately. 4. Perform mesotomicro stress amplifications (see Eq. 2.15). The mesoscopic stresses in fiber yarn are transferred into microscopic stresses in the fiber and epoxy matrix. 73
101 Chapter 2: Multiscale Modeling Approach 5. Apply failure criterion to predict the damage initiation. The TsaiHa theory is used to predict the damage initiation of fiber and matrix separately. A modified von Mises criterion (as shown in Eq. 2.25) is used to capture the matrix damage in both resin pocket and fiber yarn, whereas fiber failure is determined by the Maximum Stress criterion (Eq. 2.24). 6. Deploy the degradation models to the damaged element. When the damage initiation is predicted, a damage tensor d is used for the stiffness reduction of damaged element according to the indicated damage mode. In addition, a softening factor n s is used for the linear softening behavior. The stresses in the macroscopic model are thus updated for current increment and the evolution of the damage can be predicted (see Eq and Eq. 2.35). 74
102 Chapter 2: Multiscale Modeling Approach Figure 2.13 Flowchart of the progressive failure analysis implementation 75
103 Chapter 2: Multiscale Modeling Approach 2.5 Conclusion The algorithm of the multiscale modeling approach is elaborated in this chapter. The twoway information transfer scheme based on material property homogenization and stress amplification is also discussed. Based on that, a code for progressive failure analysis of textile composites across different length scales is developed. This code can perform stress amplification, failure prediction and stiffness degradation. The MMF criterion is applied in this study, which can offer the failure information at micromechanical level. The advantage of MMF is that it determines not only the stress level of damage onset, but also the position within the RVE where the damage has occurred. It is useful when the damage mechanisms are complex. For example, in the textile composite the failure modes need to be distinguished explicitly at fiber, fiber yarn or matrix phase so that corresponding stiffness reduction factor can be applied. The continuum damage mechanics (CDM) model is applied and presented in this chapter. The stiffness is degraded, not by a constant ratio but continuously according to the current stress state. This method relates the energy release rate and the crack opening to the loadcarrying capability of the damaged element based on the concept of fracture mechanics. The damage tensor is used to perform the stiffness reduction according to the identified damage mode. A softening factor is used as well to model a linear softening postfailure behavior. 76
104 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Chapter 3 Progressive Failure Analysis of Plain Woven Composites 3.1 Modeling Strategy The plain weave is the simplest form of woven textile structure. Plain woven based composite materials are of much interest in the applications subject to outofplane loads, due to the high delamination and impact resistance. A road map is presented for the failure analysis of plain woven composites within the framework of multiscale modeling approach. It consists of the following steps: 1. Build the geometrical model of the microscale RVE to represent the microstructure of the fiber yarn. Here, two fiber arrangement types are modeled: square and hexagonal. 2. Implement the micromechanical FE analysis based on its geometrical model. Sixboundary problems are resolved with the periodic boundary constraints. The simulations predict the effective material properties of fiber yarn in the woven composites. In addition the mesotomicro stress amplification factors are determined by extracting the stress states on the prescribed reference points. 3. Build the geometrical model of the mesoscopic plain woven structure. In the first place, mathematical topology of the plain woven structure is established based on 77
105 Chapter 3: Progressive Failure Analysis of Plain Woven Composites appropriate assumptions. Then, the topology is translated into the geometry of the fiber yarn and the composited resin pocket where the dimensions are determined by measuring the composite specimens under microscope. 4. Implement the mesomechanical analysis using finite elements. They provide prediction on the effective material properties of the plain woven composites. Moreover, the macrotomeso stress amplification factors are also computed. 5. Carry out the macromechanical analysis with an openhole plain woven laminated composites under a quasistatic axial tension. The ultimate tensile stress and the damage patterns are predicted through the progressive failure analysis. 6. Concurrently, conduct experiment to verify the simulation results. The multiply plain woven composite laminates are made using vacuum assisted resin transfer molding (VARTM). Tensile test is carried out according to ASTM standard D3039 [156]. 3.2 Micromechanical Model The idealized periodical representative volume element (RVE) consists of individual matrix and fibers modeled in a threedimensional space. In the microscale model, fiber is defined as a transversely isotropic material while the matrix is modeled as an isotropic material. Here, two RVEs are used to represent different fiber arrangements: square and 78
106 Chapter 3: Progressive Failure Analysis of Plain Woven Composites hexagonal (see Fig. 2.8). They both assume a uniform packing of the carbon fibers in the yarn. The volume fraction V f occupied by the fiber is 65% in the microstructure. It is calculated using the equation below, V f N d f 4A y 2 f (3.1) Where N f is the number of filament in a yarn and d f is the fiber diameter. They are predefined by the fiber manufacturer (N f is 3000 and d f is 7μm ). A y is the cross section area of fiber yarn, which is acquired from the composite specimens measurement (the measuring is elaborated in the next section). T300/epoxy (EPICOTE 1004) is used as the material system of plain woven composites. The mechanical properties of the raw materials (fiber and epoxy resin) are listed in Table 3.1 and Table 3.2, respectively. The subscript 1 of the material property refers to the fiber direction whereas 2 and 3 stand for the direction transverse to the fiber. In Table 3.1 the values of fiber longitudinal modulus + E f11 and tensile strength S f11 are provided by the manufacturer. Thereafter, the values not provided by the vendor are selected from [157] because it gives the closest values of E f11 and S + f11 (210 GPa and 3530 MPa, respectively) to the manufacturer s data (230 GPa and 3560 MPa, respectively). The material properties of epoxy resin in Table 3.2 are based on the manufacturer s specification sheet. All of those material properties are used as the input data of the microscopic models. 79
107 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Table 3.1 Material properties of carbon fibers (T300) Properties Values E f11 (GPa) 230 E f22 (GPa) 15 E f33 (GPa) 15 G f12 (GPa) 27 G f23 (GPa) 7 G f13 (GPa) 27 ν f ν f ν f Longitudinal tensile strength S f11 (MPa) Longitudinal compressive strength S f11 (MPa) 3560 Table 3.2 Material properties of matrix (Epoxy EPICOTE 1004) Properties Values E m (GPa) 3 G m (GPa) 1.11 ν m 0.35 Tensile strength S + m (MPa) 25 Compressive strength S  m (MPa) 100 Shear strength S shear m (MPa) 100 Here, unit displacements in three cases of normal deformation and three cases of shear deformation are deployed in the micromechanical analysis. The periodic nodal displacement constraints (BC1 through BC6 defined in Table 2.1) are applied. For each boundary condition, local stress distributions in the microscopic RVE can be obtained. The typical stress contours are depicted in Fig. 3.1 and Fig From the average stresses and strains, the effective stiffness matrix C can be obtained (see Eq.2.11). The compliance matrix S for the periodic RVE is thus determined by inversing the stiffness 80
108 Chapter 3: Progressive Failure Analysis of Plain Woven Composites matrix. So the compliance matrices for both square and hexagonal models (S square and S hexagonal, respectively) are determined as, S square C 1 square GPa 1 (3.2) S hexagonal C 1 hexagonal GPa (3.3) 1 For orthotropic material, the relations between the components of compliance matrix S ij and effective material properties are, E E E 1 S 1 G S11 S11 2S44 1 S 1 G S22 S11 2S55 1 S 1 G S33 S22 2S66 (3.4) Based on the Eq. 3.2 to Eq. 3.4, the values of Young s modulus, Poisson s ratio and shear modulus are calculated (see Table 3.3) which represent the effective material properties of fiber yarn. The material properties calculated based on rule of mixture are also 81
109 Chapter 3: Progressive Failure Analysis of Plain Woven Composites outlined in Table 3.3 which agree well with the simulation results. Note that there is a larger discrepancy in the value of ν 23 rather than the other properties. In fact, the calculated value of ν 23 is obtained from the transverse tensile modulus E 22 and shear modulus G 23. The difference between the calculated and predicted value is because the assumptions in the inverse rule of mixture for E 22 and G 23 calculation become invalid in the micromechanical FE model. In the inverse rule of mixture, identical average stress over the fiber and matrix domains is assumed however in the present FE models, neither stress nor strain over the fiber and matrix domains is consistent. Figure 3.1 Local stress contours in square microscale RVE: (a). Longitudinal axial stress σ 11 under BC1; (b). Transverse axial stress σ 33 under BC3; (c). Longitudinal inplane shear stress τ 13 under BC5; (d). Transverse shear stress τ 23 under BC6 82
110 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.2 Local stress contours in hexagonal microscale RVE: (a). Longitudinal axial stress σ 11 under BC1; (b). Transverse axial stress σ 33 under BC3; (c). Longitudinal inplane shear stress τ 13 under BC5; (d). Transverse shear stress τ 23 under BC6 Table 3.3 Predicted effective properties of fiber yarn Properties Square RVE Hexagonal RVE Rule of Mixture E 11 (GPa) E 22 (GPa) E 33 (GPa) G 12 (GPa) G 13 (GPa) G 23 (GPa) ν ν ν In addition, the mesotomicro stress amplification factors are calculated through this micro analysis. Reference points are separately selected at fiber and matrix phase with prescribed arrangement in Fig.2.9. The typical mesotomicro stress amplification factors 83
111 Chapter 3: Progressive Failure Analysis of Plain Woven Composites and their corresponding reference points are enumerated in Fig. 3.3 and Fig It is noted that there is no failure involved in the micromechanics, and the material linearity is presumed. Therefore, the values of the stress amplification components are constant in the given material system. These data are extracted and used in the failure analysis at larger length scales to capture the local damages. Figure 3.3 Typical stress amplification factors and the corresponding reference points in square RVE 84
112 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.4 Typical stress amplification factors and the corresponding reference points in hexagonal RVE 3.3. Mesomechanical Model Geometric Modeling The mesoscopic RVE of plain woven composite laminate consists of two warp yarns interlaced with two weft yarns. These two fiber yarns in the plain woven structure are perpendicular to each other: weft yarn path along directionx and warp yarn path along directiony (see Fig. 3.5). The fiber yarn is modeled as a transversely isotropic part with linear elastic material properties, which are determined from FE simulation of microscale model. In addition resin pocket filling the gap between the fiber yarns is modeled as elastic isotropic material. The geometry of the plain weave structure is guided 85
113 Chapter 3: Progressive Failure Analysis of Plain Woven Composites by the measurement of the actual specimens. The plain woven laminated composites are made using vacuum assisted resin transfer molding (VARTM) with the material system of T300/epoxy resin EPICOTE Four specimens are cut and observed under the microscope. The typical micrographs are presented in Fig It is seen that the yarn cross section presents an ellipselike shape which can be described by the measured yarn thickness and width. Figure 3.5 Fiber yarns in mesoscopic RVE of plain woven composites 86
114 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.6 Cross section micrograph of the plain woven composite laminate: (a) & (b). Fiber bundle and resin rich zones images; (c). Overall view of bundle path and crosssection. Through measurement, the geometry of the fiber yarn can be characterized based on three assumptions below: 1. The cross section of the fiber yarn is assumed elliptical in shape [35]. The major axis radius is denoted by l a and the minor axis radius is denoted by l b (Fig. 3.7). It is assumed that the area and shape of the yarn cross section remain constant. The values of l a and l b are determined from the specimen measurement. 87
115 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 2. The waviness of the yarn follows the profile of cross section of the interlaced yarn. The crimp path of the centerline of the yarn is described using a parameterized function Z(X) [35]. As illustrated in Fig. 3.7, the path is divided into five segments. Z denotes the crimp height of the centerline of the yarn and X is the horizontal coordinate of the centerline. There are two curved segments (r 2 and r 4 ) which are tangential to the profile of the yarn crosssection. Three straight lines (r 1, r 3 and r 5 ) are used to represent the portion between the curved segments. The crimp path function Z(X) is expressed in Eq.3.5 [35]. 3. The matrix fills the remaining portions of the volumes between the fiber yarns. Figure 3.7 Geometry of fiber yarn 88
116 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 1 r1 : Z X X X1 2 X1 X2 X r2 : Z X 1 2 l la 3 2 r3 : Z X X X3 X2 Z ( Z Z ) X2 X3 ( ) 2 2 X3 X4 X r4 : Z X 1 2 l la 5 4 r5 : Z X X X 5 4 Z X5 X4 X (3.5) ( Z ) ( ) 2 b b The parameters for geometric modeling are determined by the image processing technique. Here, four composite specimens were measured and six cross section images were captured for each one. A program is developed in MATLAB to read the 24 micrographs and statistically calculate the dimensions. The measured results are listed in Table 3.4. Table 3.4 Geometrical paramtes measured from the specimens Properties Values (mm) l a l b (X 1, Z 1 ) , (X 2, Z 2 ) , (X 3, Z 3 ) , (X 4, Z 4 ) , (X 5, Z 5 ) ,
117 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Given this information, fiber yarn can be modeled as a 3D solid by extruding an elliptical crosssection shape along a twodimensional spline (see Fig. 3.8). The function of the spline is described in Eq.3.5. Between the interlaced fiber yarns, the solid model of resin pocket is obtained by subtracting the shape of fiber yarns from a threedimensional rectangular volume. Figure 3.8 Threedimensional Modeling of fiber yarn in ABAQUS The solid model is imported into a 3D finite element mesh model with prescribed element size as presented in Fig nd order tetrahedral element (C3D10) is used in the model. Mesh density is defined according to the geometries. For instance, finer elements are used at the weftwarp interfaces as well as yarnmatrix interfaces while coarser mesh is defined in other regions. The mesh of the whole mesoscale RVE contains elements. Another assumption is the perfect bonding at weftwarp and yarnmatrix interfaces. The pairs of elements at these interfaces are thus tied for all six degrees of freedom. 90
118 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.9 Mesoscale finite element model: (a) Whole RVE (b) resin pocket (c) fiber yarn It is recalled that the material properties of the fiber yarn are obtained from the prediction of micro analysis as shown in Table 3.3. The constitutive relations are defined according to the local coordinates considering the material anisotropy of fiber yarn where the local axes in the yarn should follow the crimp path. By incorporating FORTRAN code into the userdefined subroutine ORIENT, local orientations of material properties are defined for each fiber yarn element. Fig 3.10 illustrates the local material orientations modeled in fiber yarn, where 1axis denotes longitudinal fiber direction while 2axis and 3axis indicate the transverse directions. 91
119 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.10 Local orientations prescribed in fiber yarns Stress Analysis In this section, stress analysis of mesoscale RVE model under six boundary problems is performed. The applied boundary conditions are the same as those used in the micro analysis. One of the objectives of the meso stress analysis is to predict the effective overall material properties of the mesoscale RVE model. The results are also used in the macroscopic analysis of composite structures. As presented in Table 3.5, the plain woven laminated composites exhibit orthotropic characteristics. It is noted that no significant difference exists between the predicted material properties for square micro model and hexagonal micro model. In addition, the inplane Young s modulus E xx and E yy are almost the same due to the identical reinforcements of weft and warp yarns in xaxis and yaxis, respectively. Those predicted inplane tensile modulus and Poisson s ratio are validated by the experimental data in section 3.5. As a result, the predicted longitudinal tensile 92
120 Chapter 3: Progressive Failure Analysis of Plain Woven Composites modulus E xx agrees well with the experimental data (see experimental validation in section 3.3.4). The properties predicted from hexagonal model are used in the following analysis because it shows better proximity with experimental data than the square model (although the difference is very small). Table 3.5 Predicted effective properties of mesoscale RVE model Properties Square RVE Hexagonal RVE E xx (GPa) E yy (GPa) E zz (GPa) G xy (GPa) G xz (GPa) G yz (GPa) ν xy ν xz ν yz The macrotomeso stress amplification factors are computed as well based on the meso stress analysis. The first step is identifying the reference points within the mesoscopic model. To obtain a complete set of reference points, local stress concentrations under all six boundary conditions are investigated. They are separately identified within the fiber yarn and resin pocket. Different local stress components are used to determine the critical region within the fiber yarn as demanded by its anisotropic feature. On the other hand, resin pocket is regarded as isotropic material, so failure criterion for isotropic materials (such as von Mises criterion) can be used to identify the critical regions. In this study, the matrix damage index D MMF is used to conduct critical region identification. This index is 93
121 Chapter 3: Progressive Failure Analysis of Plain Woven Composites calculated subject to a modified von Mises criterion applied in MMF theory (Eq. 2.25) that takes into account the difference between tensile strength S + and compressive strength S  of epoxy matrix. The stress analysis results can be presented as stress contours (see Fig through Fig. 3.18). For example, Fig illustrates that stress concentrations σ 11 (σ 11 denotes the stress component along the path of fiber yarn) locate at the crimp region of the yarn when it is under the longitudinal tension (BC1). Fig exhibits the stress distributions in fiber yarns under inplane shear, which reveals that high stresses occur at the edge of the yarn interlacing area. In addition, critical regions within the resin pocket are identified by index D MMF, which shows consistent stress concentration area within the yarns. Stress analysis under outofplane deformation (outofplane tension BC3 and outofplane shear BC5) is performed where stress concentrates are observed at yarn crimp and interlacing regions (see Fig, 3.15 to Fig. 3.18). These figures also illustrate the reference point identification under different loading conditions. It is seen that the arrangement of reference points closely follows the stress distributions on the mesoscopic model. They are chosen according to following rules: 1. The selected references points must be able to represent the critical regions at high stress levels (within top 0.5% of all nodes). 94
122 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 2. To reduce the computational cost, for each symmetric pair only one node is selected. For example, when the node at top surface is selected, the one at bottom surface locating at symmetrical position will be exempted. As a result, 232 nodes are selected as reference points with 76 nodes for each yarn and 80 nodes for resin pocket. Figure 3.11 Reference points in yarn under BC1 based on local stress σ
123 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.12 Reference points in resin pocket under BC1 based on D MMF. Figure 3.13 Reference points in yarn under BC4 based on local stress τ
124 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.14 Reference points in resin pocket under BC4 based on D MMF. Figure 3.15 Reference points in yarn under BC3 based on σ
125 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.16 Reference points in resin pocket under BC3 based on D MMF. Figure 3.17 Reference points in yarn under BC5 based on τ
126 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.18 Reference points in resin pocket under BC5 based on D MMF. Typical macrotomeso stress amplification factors are enumerated here for different components, i.e. weft yarn, warp yarn, and resin pocket: In the weft yarn (at node 152), we have the stress amplification matrix M, 152 mm M 152 mm (3.6) 99
127 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Where 152 indicates the node number of the selected reference point and mm denotes the macrotomeso stress transfer. In the warp yarn (at node 76564), we have the stress amplification matrix M, mm M mm (3.7) Finally, in the resinrich zone (at node 78110), we have the stress amplification factor M, mm M mm (3.8) Progressive Failure Analysis In this section, failure analysis is implemented for the mesoscale RVE under a uniaxial tension along weft yarn path. For each loading step, the stress analysis is performed based on the current nodal displacements. The stress components acting on the element of the 100
128 Chapter 3: Progressive Failure Analysis of Plain Woven Composites resin pocket are used to capture the matrix damage. Concurrently, the yarn stress states are transferred into local micro stress at both fiber and matrix phase. Mesotomicro stress amplification factors acquired from micro analysis are used here for the stress transfer. Thus, the microscopic fiber stress can be computed to determine the fiber fracture while the matrix damage within the fiber yarn can be captured by microscopic matrix stress. In addition, material property degradation factors d ij discussed in section are deployed here to define the stiffness reductions for different damage modes. The values of degradation factors are outlined in Table 3.6. The gradual stiffness reduction scheme is also modeled with fracture properties presented in Table 2.2. Table 3.6 Degradation factors for all damage modes in mesomechanical analysis Degradation Factors Fiber Failure Matrix Failure within yarn Matrix Failure in Resin Pocket d d d d d d The results from the meso failure analysis are presented and discussed here. Firstly, the damage patterns are illustrated in Fig to It is seen that matrix damage initiates at the crimp regions at both weft and warp yarns under applied strain 0.12% (see Fig. 3.19a). As shown in Fig. 3.19b, matrix damage in resin pocket occurs immediately after the damage onset in the yarns (at applied strain 0.15%). The damage propagations are illustrated in Fig.3.20 where extensive matrix damages exist in warp yarn while less matrix damages occur in the resin pocket and weft yarn. It reveals that the matrix damages propagate faster in transverse oriented yarn, when the composite structure is 101
129 Chapter 3: Progressive Failure Analysis of Plain Woven Composites under longitudinal tension, rather than extends to the other regions. Fig presents the damage patterns at the fiber failure initiation (under applied strain 1.08%). It illustrates that fiber damage initiates at the crimp regions of weft yarns. At that time, extensive matrix damages are found in both weft and warp yarns. Fig. 3.21b exhibits the damage patterns in resin pocket when first significant load drop occurs (under applied strain 1.16%). Figure 3.19 Matrix damage initiation modes in: (a) fiber yarns (ε xx =0.12%); (b) resin pocket (ε xx =0.15%). 102
130 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.20 Damage evolution of matrix in: (a) fiber yarns (ε xx =0.3%); (b) resin pocket (ε xx =0.3%). Figure 3.21 Damage patterns at: (a) fiber failure initiation in weft yarns (ε xx =1.08%); (b) first significant load drop in resin pocket (ε xx =1.16%). 103
131 Chapter 3: Progressive Failure Analysis of Plain Woven Composites The stressstrain relation is presented in Fig where the predicted damage initiations are also labeled. It is seen that the damage onset of matrix first occurs in the fiber yarns followed by the matrix failure in resin pocket. This linear stressstrain curve shows that the matrix damage initiations at small strain level (0.12%0.15%) have limited effect on the longitudinal tensile modulus. The significant stiffness reduction (at applied strain 1.16%) is caused by the fiber failure (initiating at applied strain 1.08%) in the weft yarn. It is also noted that, after the first load drop, the residual tensile stiffness remains at a smaller level before reducing to zero. It can be explained by Fig. 3.22b where the damage accumulation is unsaturated in resin pocket at strain level for the first significant load drop. The undamaged elements in the resin pocket still have certain load carrying capability prior to the final fracture of the composite structure. Another possible reason is the application of graduate stiffness reduction scheme by which the stiffness of the failed element does not drop to zero instantaneously but gradually reduce with a liner softening behavior. Both of above reasons could contribute to the nonzero residual stiffness after the first load drop. Finally, the final failure of mesoscale model occurs when applied strain reaches to 1.45%. 104
132 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.22 Longitudinal stressstrain relation based on meso failure analysis Validation by Experiment Prior to the macro analysis, the mesoscale failure analysis is validated here by experiment. This experiment includes a group of unnotched plain woven composite samples tested under a uniaxial tension. The tested composite laminates are made with an EPICOTE 1004 epoxy resin reinforced by carbon fiber yarn T3003K, which are the same as used in the numerical analysis. Epoxy resin is infused into the fabrics by the vacuum assisted resin transfer molding (VARTM) to make the composite samples. The configuration of VARTM system is introduced in Fig The resin and hardener is first mixed together and then infused into the plain woven fabrics through a Polyethylene 105
133 Chapter 3: Progressive Failure Analysis of Plain Woven Composites tubes. Another Polyethylene tube is used as air suction tube, which is connected to the vacuum pump via a vacuum reservoir. After 24hours running of vacuum pump, the resin penetrates into the fabrics and forms the composite panel. Four specimens are cut from the composite panel by water jet cutting machine. The dimensions of the samples are 200mm 24mm 1.2mm. Tensile test is conducted on an INSTRON 8501 machine at a constant displacement rate of 2mm/min. The specimen preparation and experiment implementation follow the ASTM standard D3039 [156]. Extensometer is also used to measure the strain of the samples with the initial distance of 25mm (see Fig 3.24). It is noted that, all the stress and strain presented in this thesis, either from experiment or simulation, are engineering values. Stress is obtained from the resultant force divided by the original crosssection area. Experimental strain refers to the average strain value over the gauge length of 25 mm as well as the simulation one. Figure 3.23 Configuration of the VRTM system 106
134 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.24 Experiment setup with extensometer The stressstrain curves from the tensile test are presented in Fig. 3.25, which exhibits consistent mechanical linearity for all tested unnotched specimens. From the stressstrain relations, tensile modulus can be extracted. Also, ultimate tensile stress is obtained from the maximum stress level and the corresponding strain is regarded as the failure strain. The test results are summarized in Table 3.7. It is seen that the predicted longitudinal modulus from both square and hexagonal RVEs (39.07 GPa and GPa, respectively, see Table 3.5) agree well with the tested tensile modulus (37.38 GPa, see Table 3.7). The predicted ultimate tensile stress and the failure strain are also validated here and they are both coincident with the test results. It is found that the predicted tensile strength ( MPa) is 5.5% lower than the test result whereas the failure strain from simulation (1.16%) presents 8.95% underestimation. 107
135 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 3.25 Comparison of the stressstrain relations between simulation and experiment Table 3.7 Experimental and simulation results for plain woven composites Inplane Young's Ultimate tensile stress Sample No. Modulus (GPa) (MPa) Failure strain (%) Experiment (Mean) Simulation The damage patterns of the unnotched samples are also investigated. It is observed that the samples are broken with a brittle fracture surface (as shown in Fig. 3.26a). To get a better damage investigation, the tested specimens are observed under a microscope. The captured micrographs are presented in Fig. 3.26b which exhibit fiber breakage in the weft yarn (along tension direction) and fiber splitting in the warp yarn (parallel to the tension 108
136 Chapter 3: Progressive Failure Analysis of Plain Woven Composites direction). The latter is caused by the transverse matrix damage due to the longitudinal tension. Both of them have been successfully predicted by the meso failure analysis (see Fig to Fig. 3.21). In addition matrix damage are observed as cracks within resin pocket (see Fig. 3.26b). This damage mode is successfully predicted by the FE simulation. (a) (b) Figure 3.26 Failure pattern of tested unnotched specimen 109
137 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 3.4. Macromechanical Model FE Modeling In this section, the FE based macro failure analysis developed in Chapter 2 (see the flow chart in Fig. 2.13) is performed for fourlayer plain woven composite laminates. Because the composites structure contains fastener holes in many applications, openhole tension (OHT) problem is solved in the macromechanical analysis. FE model for the 3D macroscopic composite part is created with the dimensions of 200mm 24mm 1.2mm (see Fig. 3.27). A 4 mm diameter central open hole is made according to the suggested diameter to width ratio (which is 1 6 ) in ASTM standard D3039 [156]. 2nd order tetrahedral element (C3D10) is used here with minimum element size 0.2mm. The material properties of the macro model are acquired from the elastic constants of overall mesoscopic model (as shown in Table 3.5). 110
138 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.27 Macroscale FE model for OHT problem To generate progressive damage patterns, quasistatic tension is applied upon the model along the longitudinal direction (xaxis). The damage modeling techniques developed in section 2.3 is applied here for stiffness reduction of failed element. Blackketter s stiffness degradation model [127] is used here which classified the degradation factor d according to different failure modes. Those degradation factors values have been suggested in [111] for progressive failure analysis of graphite/epoxy plain woven composite laminates (as listed in Table 3.8). The continuum damage mechanics (CDM) is modeled with the combination of degradation factor d and softening factor n s (see Eq and 2.35). 111
139 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Table 3.8 Degradation factors used for different damage modes in macro analysis [111] Degradation Factors Fiber Failure Matrix Failure within Yarn Matrix Failure within Resin pocket d d d d d d Simulation Result Fig presents the progressive damages predicted by FE simulation. These results exhibit the evolution of the accumulated damage when the macroscopic model is under uniaxial tension: 1. The matrix failure in fiber yarn initiates from the edge of open hole at the strain level around 0.08%. 2. Then, the matrix failure starts to propagate along the width direction until the onset of fiber damage is observed at the strain level of 0.5%. 3. Matrix damages become extensive as the strain level approaches 0.73%. 4. The maximum tensile stress occurs at the strain level of 1.49% with a narrower band of fiber failure, and a wider band of matrix failure. 112
140 Chapter 3: Progressive Failure Analysis of Plain Woven Composites 5. The final failure (residual stiffness reduces to zero) of the macro model is predicted when it is loaded under the strain of 2.75%. The stressstrain relation is presented in Fig 3.29 with the progressive damage patterns labeled accordingly. The distribution of longitudinal elastic stress s 11 is also presented in this figure. The simulation results are validated by the experimental data in the next section. Figure 3.28 Progressive damage patterns predicted from macro failure analysis 113
141 Chapter 3: Progressive Failure Analysis of Plain Woven Composites Figure 3.29 Longitudinal stressstrain relation from Macro FE analysis with CDM modeling Validation by Experiment In this section, a group of plain woven composite samples with a centralopen hole are tested to verify the macroscopic analysis result. The composite laminates are made with the same material as used in the FE simulation. Here, five specimens are cut from the composite panel by water jet cutting machine. Same as macroscopic model, the dimensions of the samples are 200mm 24mm 1.2mm. A 4mm diameter open hole is made in the center of each specimen (see Fig. 3.30). The experiment procedure is the same as the tensile test conducted for unnotched specimens. Extensometer is used as well to measure the strain of the samples with the initial distance of 25mm. Longitudinal strain 114
142 Chapter 3: Progressive Failure Analysis of Plain Woven Composites is measured from the displacement over the gauge length divided by the original gauge distance (also see Fig. 3.30). Figure 3.30 Untested plain woven OHT specimen The stressstrain curves from the tensile test are presented in Fig. 3.31, which exhibits nonlinear responses for all tested OHT specimens. Ultimate tensile stress is extracted from the maximum stress level of each sample. The experimental results are outlined in Table 3.9. Results from numerical analysis are compared here with the experimental data. To demonstrate the effect of CDM modeling on the tensile strength prediction, another FE analysis is performed with instantaneous stiffness reduction method where the soft factor n s is not used (as shown in Eq and Eq. 2.29). It is illustrated that the developed model can predict consistent ultimate tensile stress with the experimental result (279.8MPa) if the gradual stiffness reduction method is applied (301.2 MPa) whilst the macro failure analysis with instantaneous stiffness reduction scheme only can predict 115
143 Chapter 3: Progressive Failure Analysis of Plain Woven Composites about 80% (223.5MPa) of the experimental tensile stress. In other words, the soften factor n s has strong influence on the tensile behavior prediction of plain woven composites, which provides 34% increase of predicted ultimate tensile stress in the current material system. Figure 3.31 Comparison of results between FE simulation and Experiment Table 3.9 Tensile test results for plain woven composites Inplane ultimate tensile stress Sample No. (MPa) Experimental Mean Data Simulation with Gradual Stiffness Reduction Simulation with Instantaneous Stiffness Reduction
144 Chapter 3: Progressive Failure Analysis of Plain Woven Composites In addition, the predicted damages mechanisms are validated against the tested OHT specimens. The captured micrographs presented in Fig exhibit a nonuniform damage patterns along the fracture surface where some fiber pullouts are observed in the vicinity of the central hole whereas the fracture far away from the central hole remains brittle and neat (see Fig. 3.32b). This phenomenon proves the occurrence of the fibermatrix debonding. The fibermatrix debonding cannot be captured in current failure analysis because this damage mode is not established in the developed multiscale modeling. It is noted that accurate prediction of fibermatrix debondings highly depends on the fibermatrix interface parameters. Unfortunately, those parameters cannot be precisely determined in our current experimental setup. In addition, it is seen that the predicted stiffness only agrees well with the test result at the small strain level (< 0.15%). To have a better understanding for the present modeling approach, a comprehensive sensitivity study is performed and outlined in Table It presents that the fiber elastic properties have dominant influence on the tensile behavior of plain woven composites. Then, the damage behavior is highly affected by the textile geometries. It is also noted that, with deploying the continuum damage mechanism, the ultimate tensile stress is significantly dependent on the Mode I Fiber fracture toughness. At last, various selection range of reference points for macro/meso stress amplification are studied. It shows that the mechanical performance doesn t rely on the selection ranges (0.1% to 1%). Therefore, for the inconsistent response of the experimental specimen appears and the predicted one, the possible reason could be: Firstly, insufficient prediction of failure modes (e.g. fiber pullouts). One of the possible reasons for the difference between prediction and experiment is, in this thesis, three essential failure modes are well defined and can be determined in the failure analysis fiber fracture, epoxy damage within yarn, epoxy damage in the 117
145 Chapter 3: Progressive Failure Analysis of Plain Woven Composites resinrich zones. However, it is not necessary to limit the failure analysis within those three failure modes. More failure modes can be defined in this multiscale framework and provide more accurate results such as fiber kinking, fiber pulling, etc. But it is noted the precise prediction highly relies on the characterization of micromaterial properties related to the damage modes. Secondly, nominal value of Mode I Fiber fracture toughness rather than the measured value is used which may be different with the actual specimen s property. Table 3.10 Sensitivity study for plain woven composites analysis Category Item Influenced object Sensitivity Geometric Modeling Material Parameters Crimp region in woven composites Stress distribution Strain localization Damage initiations High Elastic Stiffness of fiber Longitudinal tensile behavior Dominantly Mode I Fiber fracture Ultimate tensile strength for High toughness longitudinal tension Selection range of reference points Damage initiation Low (a) 118
146 Chapter 3: Progressive Failure Analysis of Plain Woven Composites (b) Figure 3.32 Tested plain woven OHT specimen 3.5 Conclusion In this chapter, the hierarchical multiscale modeling approach is applied in the study of plain woven composite material. Progressive failure analysis based on this multiscale modeling provides accurate predictions of mechanical performance laminated composites. The presented approach includes hierarchical numerical simulations on repeated RVEs at micro and meso length scales, and macroscopic OHT laminates. The analysis starts from the micromechanics, where the effects of reinforcement volume fraction, spatial distribution, and the properties of constituents (fiber and matrix) are taken into account. Six periodic boundary problems are solved to obtain the effective yarn stiffness and the stress amplification factors. The stress amplification factors are calculated based on the prescribed reference points. Mesomechanical analysis accounting for plain woven architecture is conducted to provide effective material properties and macrotomeso stress amplification factors. The mesoscopic failure analysis is also 119
147 Chapter 3: Progressive Failure Analysis of Plain Woven Composites performed to investigate the progressive damage response of unnotched plain woven laminated composites under uniaxial tension. Finally, the macroscopic OHT problem is solved based on developed multiscale modeling approach to predict the progressive failure behavior. Here, the multiscale damage modes are determined by applying TsaiHa theory where Maximum Stress criterion is used for fiber failure and a modified von Mises criterion is used for matrix damage. Damage evolutions are modeled with a continuum stiffness reduction scheme for all damage mechanisms. Simulation results obtained from the failure analysis are also verified by the tensile test. Consequently, the simulations can predict accurate tensile behaviors of plain woven composites regardless of unnotched or OHT laminates. The experimental validation exhibits that the effective material properties can be determined based on the constituent material properties (fiber and matrix) through the stiffness homogenization method. It is also proven that the soften factor n s applied in CDM significantly affects the predicted tensile behavior of plain woven composites. It shows that CDM can provide more accurate prediction on ultimate tensile stress than the instantaneous stiffness reduction model. Furthermore, both numerical and experimental studies reveal that final fracture of the plain woven composite is dominantly attributed to the fiber failure in longitudinal yarn and matrix damage in transverse yarn. Finally, the present multiscale modeling approach predicts a lagging occurrence of nonlinear response comparing to the experimental result. The possible reasons of this difference have been discussed as well. 120
148 Chapter 4: Progressive Failure Analysis of NCF Composites Chapter 4 Progressive Failure Analysis of NCF Composites 4.1 Introduction to NCF Composites Textile fabric based composites have been developed to improve the outofplane properties and reduce manufacturing cost. However, the crimp of the fiber yarns in the textile composites leads to deterioration of the inplane performance especially in compression. To overcome that problem, NCF composites have been proposed. They consist of UD plies arranged in different directions while the fibers are consolidated by the stitches within each ply. The advantages of NCF composite laminates over the conventional UD laminates are outlined as follows: 1. NCF composites provide superior outofplane properties owing to the throughthickness reinforcement of stitches. For example, it has been proven that stitching enhances both mode I and II energy release rate [41, 42]. 2. NCF composites have higher impact resistance. The compression after impact (CAI) strength increases through stitching in NCF composites [37]. 3. The layup time of the stitching fabrics is dramatically reduced because they are produced in one step only [4]. 121
149 Chapter 4: Progressive Failure Analysis of NCF Composites 4. The NCFs can be handled easily in composite production and thus are capable of making complex shapes. In addition NCF composites offer superior inplane mechanical performance to other textile composites (e.g. woven and braided composites) because nocrimp fiber yarn can contributes more reinforcement along the longitudinal direction. On the other hand, the needle insertion during the stitching process causes fiber displacement. It may result in misalignment, discontinuity, breakage and crimp of fibers [4, 40, 49, 50]. Those disturbances induce the formation of resin pocket in the stitch vicinity which affects the stress distribution and damage behavior of NCF composite structure [36, 5053]. In this chapter, the progressive failure analysis of NCF composites is implemented. The multiscale modeling approach applied for plain woven composite (in Chapter 3) is further developed here. This modified method can accomplish following new tasks: Firstly, a nonlinear multiscale modeling approach is developed where the material nonlinearity of epoxy resin is taken into account. The nonlinear modeling is the new research interest to study the nonfiberdominated mechanical behavior of textile composites. Choosing NCF for the nonlinearity study is because: 1. There is proven MesoFE modeling method developed for the mechanical analysis of multiaxial NCF composite [50, 51]. 122
150 Chapter 4: Progressive Failure Analysis of NCF Composites 2. Basically, there are two nonlinearities involved in the mechanical nonlinearity study of composites, geometry and material nonlinearity. In this thesis, the study of interest is to explore the influence of matrix material nonlinearity on the mechanical behavior of textile composites. The effect of the geometry nonlinearity should be minimized here so that the predicted nonlinear stressstrain curve will highly depends on the nonlinear material properties. Therefore, NCF is selected here because the fiber yarns in NCF present less crimp and lead to less geometric behavior than the other textiles. In addition, to consider the effect of the stitching, the resinrich voids created by needle insertion are included in the mesomechanical modeling of NCF laminated composites. The stitches are also represented by adding nonlinear spring elements to the FE models with prescribed stitching parameters. Besides, interlayer delamination is taken into account in this chapter. The tractionseparation constitutive law is used for the cohesive interactions between the layers. Based on the considerations above, progressive failure analysis is individually conducted for 0 degree, biaxial, and quasiisotropic NCF laminates. 4.2 Nonlinear Mechanical Modeling of NCF composites In this section, a modified version of multiscale modeling approach is presented, which involves two nonlinear modeling techniques: 123
151 Chapter 4: Progressive Failure Analysis of NCF Composites 1. The prefailure nonlinear behavior of epoxy resin is modeled into the material system. A simple elasticplastic constitutive model is developed in section The TsaiHa theory is modified here to perform nonlinear stress amplification across different length scales that can capture the variation of stress distribution during the plastic yielding (see section 4.2.2) Modeling of Elastoplasticity for Epoxy Resin Accurate stress analysis relies on the correct constitutive modeling of the materials. For composite materials, different components can exhibit different material characteristics. Usually, carbon fiber is treated as a linear elastic material whilst the epoxy resin could contribute certain nonlinearity to the overall composites performance. Generally speaking, linear elastic modeling is adequate to predict the fiberdominated mechanical behaviors of composite laminates (e.g. the longitudinal tensile modulus and longitudinal tensile strength). On the other hand, a number of researches revealed that the material nonlinearity of the resin epoxy influences the stress distributions and damages in the composite laminates [27, 107]. As early as in 1987, Chang and Chang [107] reported that the material nonlinearity was important to predict the damage in composite laminates under shear deformation. This statement was verified by Vogler s experimental study [27]. Vogler and his colleagues developed a 3D micro RVE model to precisely predict the nonlinear shear response of carbon/epoxy composite laminates. In their study, the isotropichardening plasticity of epoxy matrix was extracted from a torsion test on a filament wound thinwalled epoxy tube. In addition, Truong et al. [89] conducted a series 124
152 Chapter 4: Progressive Failure Analysis of NCF Composites of uniaxial tensile tests for biaxial carbon/epoxy NCF composites: [0/90] ns and [ 45] ns layouts. The experimental results presented a linear stressstrain curve for [0/90] ns laminates and nonlinear response for [ 45] ns laminates (as shown in Fig.4.1). It was reported that the nonlinearity was attributed to the material plasticity of epoxy matrix when the inplane shear load was applied (in the case of [ 45] ns laminates). Likewise, Pinho et al. [137] implemented an explicit FE analysis to underline the importance of modeling the nonlinear matrix shear behavior for accurate failure prediction in the biaxial laminated composites [ 45] s under a uniaxial tension. Figure 4.1 Uniaxial tensile test results for (a) [0/90] ns NCF laminates; (b) and (c) [ 45]ns NCF laminates [89] In this section, a simple incremental constitutive model is derived to describe the prefailure nonlinear behavior of epoxy matrix. The developed elastoplasticity model can be 125
153 Chapter 4: Progressive Failure Analysis of NCF Composites easily defined into the FE analysis by writing the incremental nonlinear constitutive relations into ABAQUS  UMAT subroutine as FORTRAN language Elastoplastic Constitutive Model For the proposed elastoplastic material, the elastic and plastic behavior can be depicted separately. When the effective stress σ eff is lower than initial yield stress σ 0 y, the linear elastic stressstrain relation is written as, σ Cε (σ eff < σ y ) (4.1) e Where σ denotes the stress tensor, which is determined by the stiffness matrix C and the elastic strain tensor ε e. The symmetric stiffness matrix C for isotropic material can be written as, E(1 ) 1 1 C (1 )(1 2 ) 1 2 (4.2) (1 ) (1 ) (1 ) 126
154 Chapter 4: Progressive Failure Analysis of NCF Composites Where E is the Young s modulus and denotes the Poisson s ratio. When the effective stress σ eff exceeds the initial yield stress σ 0 y, assuming the epoxy resin as isotropic hardening material, the plastic stressstrain is given as, σ m( ε ) n (σ eff σ 0 y) (4.3) p 0 y The constants m and n are used to describe the plasticity of the isotropic hardening material. The tensor of plastic strain increments can be presented as, dε dε dε e p (4.4) Based on that, the tensor of elastic stress increments can be written as, dσ Cdε C( dε dε ) (4.5) e p Yield Function By applying the isotropic hardening rule, the general form of the yield function presents, f ( σ, ε ) ( σ) ( ε ) 0 (4.6) p eff y p 127
155 Chapter 4: Progressive Failure Analysis of NCF Composites Where the effective stress is represented by the von Mises stress eff vm (4.7) Associated Plasticity Here, the associated flow rule is applied that assumes the plastic potential function g(σ) has the same shape as the current yield surface f(σ, ε p ). Thus, the gradient of plastic potential function is equal to the direction normal to the yield surface, g f n e ff σ σ σ (4.8) Where the gradient of the plastic potential function is controlled by the effective plastic strain increment ε eff, ε n e ff (4.9) The tangent modulus H is presented as the gradient of the effective stressstrain curve and can be calculated based on Eq.4.3, ' e ff H e ff (4.10) 128
156 Chapter 4: Progressive Failure Analysis of NCF Composites Substitute Eq. 4.8, Eq.4.9 and Eq.4.10 into Eq.4.5, we can obtain the incremental stressstrain relation, T Cnn C dσ C d ' T H ε n Cn (4.11) The elastoplastic constitutive relation is then written to ABAQUS subroutine UMAT. This userdefined material system is verified in section Parameter Identification The parameters used in the elastoplastic constitutive model are determined from tensile test for the pure epoxy resin. Four specimens are tested under a uniaxial tension (see Fig 4.2) on an INSTRON 8501 machine at a constant displacement rate of 2mm/min. As described in section 3.5, the experimental procedure follows the ASTM standard D3039. Strain gauges are mounted on the sample surfaces to measure the strain values. By fitting the experimental stressstrain curves with an exponential function (see Fig. 4.3), the parameters are determined as listed in Table
157 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.2 Tensile test samples for pure epoxy resin Table 4.1 Material properties obtained from tensile test for epoxy resin samples Properties Values m (MPa) n σ 0 y (MPa) Ultimate tensile stress t S (MPa) m
158 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.3 Tensile Test results for pure epoxy resin samples Nonlinear Stress Amplification Method In the stress transfer method developed by Ha et al. [97], the constant stress amplification factors are calculated based on the prescribed fixed locations of reference point. However, using constant stress amplification factors is reasonable only when the stress distributions within the RVE model are invariable. In this study, an elastoplastic material system is developed. The stress distributions don t remain constant due to the prefailure plastic yield of epoxy matrix. The prefailure here refers to the status of the material before the crack occurs. Thus, prefailure plastic yield means the plasticity onset prior to the material fracture. A new stress amplification method is proposed in this section which can capture the variation of stress concentrations and the nonlinear globallocal stress relations due to plastic yield and fracture. 131
159 Chapter 4: Progressive Failure Analysis of NCF Composites The local and global stresses can be written as two 6 1 stress vectors, Local stress vector: σl L L L L L L T (4.12) Global stress vector: σ G G G G G G G T (4.13) Where 16 denote six loading conditions. In nonlinear stress transfer case, each of the components in the nonlinear stress amplification matrix is no more a constant but a function of global stress tensor, M( σg) M1 j ( σg) M 2 j ( σg) M3 j ( σg) M 4 j ( σg) M5 j ( σg) M6 j ( σg) T (61) (4.14) This matrix is then used to determine the local stress tensor, 6 j j L ( G ) G j ( G ) G j1 σ M σ σ M σ σ (4.15) Where M ( j ) 1 ( j ) 2 ( j ) 3 ( j ) 4 ( j ) 5 ( j ) 6 ( j j G M j G M j G M j G M j G M j G M j G) T (61) (4.16) 132
160 Chapter 4: Progressive Failure Analysis of NCF Composites Equations (4.15) and (4.16) indicate that any one column in the amplification matrix M only varies with one corresponding global loading case. Therefore, the amplification matrix M can be rewritten with the nonlinear amplification vector M ( σ ) as, j j G M( σg) M1( G) M2( G) M3( G) M4( G) M5( G) M6( G) (66) (4.17) Furthermore, the value of components in the amplification matrix can be controlled by using the nonlinear coefficient D. Based on all the equations above, the nonlinear stress amplification matrix can be expressed as, M ( ) D ( ) M j j 0 j G j G j (4.18) Where 0 M j are the constant amplification factors determined in the initial status. Then Equation (4.18) can be further rewritten as: M( σg) D1 ( G) M1 D2 ( G) M2 D3 ( G) M3 D4 ( G) M4 D5 ( G) M5 D6 ( G) M 6 (4.19) Reforming the amplification factor matrix M as a vector, D ( σ ) is the nonlinear coefficient, which is a function of global stress. Then Equation (4.19) can be reformulated as: j G 133
161 Chapter 4: Progressive Failure Analysis of NCF Composites M ( ) D ( ) M M D M M D M M D M M D M M D M G 1 G ( G) 2( G) ( G) 3( G) ( G) 4( G) ( G) 5( G) ( G) (36 1) 6( G) (3636) 6 (361) The general nonlinear coefficient matrix D( σ G) can be obtained as: (4.20) D j D( G ) 1 1( G ) D 2 2( G ) D 3 3( G ) D 4 4( G ) D 5 5( G ) D ( ) 6 6 G (36 36) (4.21) Method to Determine Nonlinear Coefficient j The method to determine the nonlinear coefficient D ( ) is discussed here. Consider six loading cases: three normal loadings and three shear loadings, respectively. In each case, only the jth component in the global stress vector is nonzero, and all other components are zero, then Equation (4.15) can be simplified as: j G σ D ( ) M j 0 j j G j G (4.22) 134
162 Chapter 4: Progressive Failure Analysis of NCF Composites j In each loading case, sufficient number of global applied loads are implemented to G obtain the relationships between the applied loads and each component of the local j G stress σ L. These relationships are just corresponding to the nonlinear j coefficients D ( ) j G. The local stresses are first extracted based on the selected j reference point with the highest local stress level. D ( ) j G are calculated thereafter based on the relationships between the global and local stresses recorded from the first step until the final fracture of the RVE model Implementation of Nonlinear Multiscale Modeling It should be noted that within the nonlinear multiscale modeling framework, the localglobal property homogenization and globallocal stress amplification method described in chapter 2 becomes difficult to implement. The conventional homogenization method is based on the linear stressstrain relations while the stress amplification method developed in HaTsai theory relies on the linear correlation between global and local stress states. Those assumptions cannot hold in the advanced nonlinear model. Therefore, the multiscale modeling is performed in this chapter through the data fitting techniques. Two types of table are generated to govern the information transfer between different length scales: One is overall stressstrain table obtained from stress analysis at smaller length scale, which is used to assign the nonlinear material properties into the elements in the larger scale FE model. Another tabular form, whereby the nonlinear stress amplification j factors are calculated, is created to correlate the nonlinear coefficients D ( ) and the j G 135
163 Chapter 4: Progressive Failure Analysis of NCF Composites j global average stress G. The tables are first prepared from the micro and meso FE simulations. Subsequently, they are deployed in the macro analysis to predict the progress failure behaviors. The details of the nonlinear multiscale modeling is elaborated in following sections. 4.3 Micromechanical Model The objectives of NCF micro analysis include predicting the effective material properties of fiber yarn and calculating the nonlinear stress amplification factors. The material system defined in the micromechanics of NCF composites includes the mechanical properties of fiber and epoxy resin. Note that same material system is used for studies of plain woven and NCF composites (T300/ EPICOTE 1004). Thus, the properties of carbon fibers (T300) in Table 3.1 are also used here. For resin rich zone, the experimentfitted nonlinear stressstrain relations (see section 4.2.1) are deployed here to model the elastoplastic material behavior of matrix. The other material properties of epoxy resin which cannot be determined from the tensile test (eg. matrix compressive strength, matrix shear strength, etc.) are taken from Table 3.2. The 3D micro FE model is presented in Fig.4.4. The hexagonal geometry is meshed with 3D 1 nd order brick element (C3D8) with a minimum element size 100nm. Six periodicdisplacement loading conditions in three cases of normal loads and three cases of shear loads are applied. For each loading condition, the occurrence of prefailure plastic yielding of epoxy matrix is predicted within the micro RVE model. Based on that, the 136
164 Chapter 4: Progressive Failure Analysis of NCF Composites nonlinear mechanical responses can be obtained. Figs 4.5 to 4.9 exhibit the stressstrain relations from micro FE analysis under different loading conditions. It is seen that the longitudinal tensile behavior is not influenced by the plasticity of matrix (see Fig. 4.5) because it is dominantly determined by fiber properties. In addition, prefailure nonlinearity responses are illustrated in Figs 4.6 to 4.8 when the RVE model is under transverse and shear deformations. The simulations are terminated when the damage onset of matrix is identified by the modified von Mises criterion (see Eq. 2.25). The failure patterns of matrix at the end of simulation are also illustrated in Fig. 4.5 through Fig Figure 4.4 Threedimensional hexagonal microscale RVE model 137
165 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.5 Stressstrain curve of micromechanical analysis under longitudinal tension Figure 4.6 Stressstrain curve of micromechanical analysis under transverse tension 138
166 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.7 Stressstrain curve of micromechanical analysis under longitudinal shear Figure 4.8 Stressstrain curve of micromechanical analysis under transverse shear One of the tasks of the microscopic analysis is to predict the effective material properties 139
167 Chapter 4: Progressive Failure Analysis of NCF Composites of fiber yarn. The stiffness matrix calculation demonstrated in section 2.12 is still applicable here to predict the effective elastic material properties. The results are outlined in Table 4.2. However, they are not adequate to describe complete prefailure mechanical behaviors if the material nonlinearity of epoxy resin is not incorporated. Thus, the localtoglobal characterization method of nonlinear material property proposed by Tserpes and Labeas [36] is deployed here. The effective nonlinear behaviors of NCF composites are determined by assigning the fitted stressstrain relations (Figs 4.6 to 4.8) from FE analysis of local RVE model into the global material points of the macroscopic structure. This semiempirical method treats the FEA as virtual experiments and uses the simulation results to govern the local mechanical behaviors. To achieve that, several lookup tables are generated to define the local modulus H for different load cases. For instance, a table (see Table 4.2) for local tangent modulus H xy under longitudinal shear is generated by extracting data from the stressstrain curve in Fig.4.7. The instantaneous local modulus H xy will be used to replace the constant elastic shear modulus G xy in the subsequent mesoscale analysis. This table also points out that the plasticity of matrix occurs at a longitudinal shear strain of %. The table ends up at the strain level of matrix damage onset (0.8991%). Local modulus for other stressstrain behaviors such as longitudinal tension, transverse tension, and transverse shear can be acquired in the same manner. 140
168 Chapter 4: Progressive Failure Analysis of NCF Composites Table 4.2 Table for local longitudinal shear modulus H xy fitting to simulation result γ xy (%) H xy (MPa) γ xy (%) H xy (MPa) γ xy (%) H xy (MPa) γ xy (%) H xy (MPa) The meso/micro nonlinear stress amplification factors are also calculated based on the micro analysis. For epoxy matrix phase, amplification factors are determined based on 141
169 Chapter 4: Progressive Failure Analysis of NCF Composites the identification of floating reference points. Here, the reference point is chosen at the node of maximum stress states within the matrix phase, which can be easily obtained from the simulation result data. Floating means the locations of the reference point vary with the stress redistributions. Fig.4.9 illustrates the floating reference point in the case of transverse tension. It shows that the node of maximum local stress states varies with the increase loading. It is also revealed that it is the plastic yielding of epoxy matrix which causes such stressredistributions. Figure 4.9 Floating reference point positions under transverse tension Based on the stress states of the floating reference points, the nonlinear stress amplification factors can be calculated following these steps: 142
170 Chapter 4: Progressive Failure Analysis of NCF Composites 1. Calculate the initial linear stress amplification matrix M 0, which are obtained at matrix phase referring to the maximum local stress states (at first load increment). 2. The relationships between the global and local stresses (on the floating reference points) are tracked and recorded from the first step until the matrix failure onset. j Thus the nonlinear coefficient D ( ) (j=16, denoting six loading cases) can be determined. j G 3. Applying Eq. 4.22, the nonlinear stress amplification matrix is obtained. For example, the initial stress amplification matrix 0 Mm in epoxy matrix region is calculated based on the stress analysis under six loading conditions. The value of 0 Mm is, M 0 m (4.23) From the FE analysis results for transverse tension problem (along zdirection), nonlinear coefficient D ( ) 3 zz is computed based on the globallocal stress relations. The global stress in this case is the average stress along the transverse direction zz. The maximum local stress state is represented here by the damage index D MFF (see E.q. 2.25). The 143
171 Chapter 4: Progressive Failure Analysis of NCF Composites variable maximum value of D MFF is tracked and recorded by the ABAQUS postprocessing tool with the plastic yielding of epoxy matrix. The relations between D MFF and zz are presented in Fig It is noted that the curve ends when the D MFF equals to 1 which identifies matrix damage initiation. Then, the table (see Table 4.3) for nonlinear coefficient D ( ) 3 zz can be generated to guide the calculation of nonlinear stress amplification factor (where the initial nonlinear coefficient defined as 1). It is found the nonlinear coefficients increase with the load increment which means the plastic yielding of epoxy resin results in the greater stress localizations within the micro model. In other word, the analysis including material plasticity of matrix predicts earlier damage onset j than the linear elastic model. The other components in D ( ) are determined by solving other loading problems. The complete nonlinear stress amplification factors are thus calculated according to Eq In addition, the stress amplification factor for fiber phase is the same as the calculation presented in Chapter 3 since it remains linear elastic. j G Figure 4.10 Predicted globallocal stress relations from micro analysis under transverse tension 144
172 Chapter 4: Progressive Failure Analysis of NCF Composites Table 4.3 Table of nonlinear coefficient D ( ) 3 zz for meso/micro stress amplification zz (MPa) D 3 zz (MPa) D Mesomechanical Model The mesomechanical analysis of NCF composites is discussed in this section, which consists of two parts: Firstly, the failure analysis for the 0 degree NCF laminate is performed. The 3D RVE model of 0ply includes the noncrimp fiber yarns and resin rich voids. The geometry of mesoscale model is characterized from the specimen measurement. This simulation needs to provide the effective material properties of NCF mesoscale model which can be used as input data for macroscopic analysis. The macrotomeso nonlinear stress amplification matrices are also calculated from this analysis. 145
173 Chapter 4: Progressive Failure Analysis of NCF Composites In addition, mechanical performance of two biaxial NCF laminates (layout [0/90] 2s and [ 45] 2s ) are also studied. Here, throughthickness stitching is represented by the nonlinear spring elements. The bilinear constitutive model of the spring element is defined based on the pullout model proposed by Zhang et al. [47] and Liu et al. [48]. Delamination is also involved in the present failure analysis by deploying the tractionseparation constitutive law in the interlayer cohesive interactions. In addition, the influence of nonlinear modeling is evaluated here through the FE analysis based on both linear and nonlinear modeling methods. Finally, the results of the performed failure analysis are validated by the experimental data Case 0 degree Laminate The mesoscale RVE model of NCF in the present study is treated as stitched unidirectional laminate with the eyes (resinrich zone due to stitching). The openings are caused by the throughthickness stitching and formed as resinrich zones in the vicinity of stitches. As presented in Fig. 4.11, the dimensions of the diamond shaped eyes are determined based on the measurement of actual specimens. The biaxial composite specimens are made of carbon NCF fabrics. The biaxial fabric consists of two plies orientated at a right angle to each other, which are integrated by the stitches. The angle between the machining direction of the stitching and the fiber yarn is 45 degree (see Fig. 4.12). The biaxial NCF composite laminates are made using vacuum assisted resin transfer molding (VARTM). The epoxy resin (EPICOTE 1004) infused into the fabric is the same as the material used in previous studies. Here, four specimens are cut and 146
174 Chapter 4: Progressive Failure Analysis of NCF Composites observed under the microscope. For each specimen, six cross section images are captured under a microscope. Then, the MATLAB code is used to process all 24 micrographs and calculate the dimensions statistically. To describe the geometry of NCF model, five geometrical parameters are defined and illustrated in Fig The measured results are outlined in Table 4.4. Figure 4.11 Parameter identification for NCF mesoscale RVE model 147
175 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.12 Top view of biaxial NCF fabric Table 4.4 Measured dimensions of NCF mesoscale RVE model Dimensions measurement (mm) Machine Distance m Cross Distance c Half Eye Length l Half Eye width d Deviation Distance n After geometrical modeling, a 3D solid model consisting of fiber yarns and resinrich zones is converted into FE mesh (see Fig. 4.13). 2 nd order tetrahedral element (C3D10) is used in this model. The material properties of fiber yarn are acquired from the nonlinear 148
176 Chapter 4: Progressive Failure Analysis of NCF Composites micromechanical analysis. The elastoplastic model developed in section 4.2 is applied here for the resinrich zones with the same material parameters used in micromechanical analysis. Figure 4.13 Import 3D mesoscale RVE geometry to 3D FE mesh Mesoscopic stress analysis is performed with six periodic loading cases. Fig presents the distributions of elastic stresses when the mesoscale RVE is under different loading conditions. It is observed that local stresses concentrate in the vicinity of the stitching locations. Here, higher local stresses 11and 13 are induced in the opening of the resinrich zones whereas 22, 12 and 23 concentrate at the tips of the diamondlike voids. 149
177 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.14 Local stress distribution in the mesoscale RVE under six periodic loading conditions 150
178 Chapter 4: Progressive Failure Analysis of NCF Composites Here, the elastic stresses are used to calculate the effective elastic stiffness of meso RVE. Nine equations presented in Eq. 3.4 are used to calculate nine independent material constants. The results are listed in Table 4.5. Note that the NCF RVE model is assumed as general orthotropic material. Therefore, the material properties are not identical along the transverse (y) and thickness (z) direction. It is also seen that, using the same material system, the predicted elastic longitudinal Young s modulus of NCF composite laminate (96.74 GPa) is much higher than in the plain woven composite laminate (37.38 GPa). That is because the noncrimped yarns in the NCF composites which can have better reinforcement along the fiber direction. The predicted effective material properties are used to describe the constitutive relations of elements in the macroscopic analysis. Table 4.5 Predicted effective elastic stiffness of mesoscale RVE model Properties Values E xx (GPa) E yy (GPa) 6.81 E zz (GPa) 8.03 G xy (GPa) 5.79 G xz (GPa) 3.58 G yz (GPa) 2.82 ν xy 0.45 ν xz 0.27 ν yz 0.21 Same as in micro analysis, the complete prediction of mechanical responses requires uptofailure nonlinear stressstrain relations under variable load conditions. Fig illustrates the elasticplastic stressstrain curves, which are used to determine the effective 151
179 Chapter 4: Progressive Failure Analysis of NCF Composites material properties of meso RVE. They will be assigned as the material properties of element in the following macro FE analysis. Figure 4.15 Stressstrain curve of meso analysis under six periodic loading conditions The meso analysis is terminated when the onsets of matrix damage are captured, which consists of two steps: resin rich zone damage and matrix damage within fiber yarn. As 152
180 Chapter 4: Progressive Failure Analysis of NCF Composites presented in Fig (a)(f), the simulations predict that the latter always occurs earlier than the former damage mode. It is also seen that the predicted damage patterns coincide with the predicted stress distributions (see Fig. 4.14) as the matrix damages initiates in the vicinity of the stitches. In particular, when xx and xz are applied upon the RVE, onset of matrix damages occur from the opening of the resinrich zones whereas when yy, xy and yz are applied, damage initiates from the void tips. The macrotomeso stress amplification factors are calculated as well in this section: Firstly, the floating reference points are tracked and extracted within fiber yarn. The initial stress amplification matrix M 0 is then calculated at the first load increment. Later, j nonlinear coefficients D ( ) are computed from the beginning up to the occurrence of j G matrix damage in fiber yarn. The nonlinear macrotomeso stress amplification factors are thus obtained through Eq The procedure is repeated to determine the stress amplification factors for resin rich zones. The initial stress amplification matrix for fiber yarn, Μ and one set of nonlinear coefficients D ( ) 2 are enumerated in Eq yarn yy and Table 4.6, respectively. 153
181 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.16 Predicted matrix damage onsets within fiber yarns and resin rich zones under six periodic loading conditions 154
182 Chapter 4: Progressive Failure Analysis of NCF Composites M 0 yarn (4.24) Table 4.6 Table of nonlinear coefficient D ( ) 2 yy for macro/meso stress amplification (MPa) yy D 2 yy (MPa) D 2 yy (MPa) D
183 Chapter 4: Progressive Failure Analysis of NCF Composites Case Biaxial Laminates In this section, two biaxial ([0/90] 2s, [ 45] 2s ) NCF composite laminates are studied. The aim of this study is to figure out the effect of the material nonlinearity of epoxy matrix on the mechanical performance prediction of NCF composite laminates. The progressive failure analysis is performed with prescribed mesotomicro stress amplification factors. In addition, the interlay delamination and stitching are considered here to provide a complete failure analysis. The geometrical models are presented in Fig (a) and (b), which are then meshed with 3D 2 nd order tetrahedral element (C3D10) in ABAQUS software. To capture the delamiantions, cohesive interactions are modeled here for interlayer contacts. The constitutive relation for the nodes between the neighboring plies is defined through the tractionseparation law. This tractionseparation behavior was applied by Ridha et al. [158] in their progressive failure of adhesive bonded composites, which can be written as: t n t s t t t n t s t t (4.25) Gn Gs Gt G c 1 (4.26) 156
184 Chapter 4: Progressive Failure Analysis of NCF Composites Where t n, t s, and t t denote the normal and shear components of tractions, respectively; t 0 n, t 0 s, and t 0 t indicate the maximum normal and shear tractions when relative displacement of the coupled nodes is in the normal or shear direction; G n, G s, and G t are the energy release rate by the normal and shear tractions, respectively; G c presents the critical total energy release rate. As presented in Eq. 4.25, the quadratic stress criterion is applied to predict the initial delamination. Linear softening tractionseparation relation is used here to describe the postfailure behavior. As shown in Eq. 4.26, the evolution of the delamination is controlled by the energy release rates [159]. However, the parameters for interlayer delamination are usually difficult to characterize unless special experiments are conducted such as doublecantileverbeam (DCB) test and threepoint bending test. Here, the material properties of matrix are used to characterize the delamination parameters (see Table 4.7). Note that the tensile and shear strength of epoxy resin are used for the maximum normal t 0 n and shear tractions t 0 s and t 0 t, respectively (see Table 3.2). Likewise, the fracture properties of epoxy resin are also used here for the energy release rate G n, G s, and G t (see Table 2.2). 157
185 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.17 Layouts of biaxial NCF laminates: (a). [0/90] 2s ; (b). [ 45] 2s Table 4.7 Parameters for interply cohesive interactions Properties Values t 0 n (MPa) 25 t 0 s (MPa) 100 t 0 t (MPa) st mode Fracture energy G nc (KJ/m 2 ) nd mode Fracture energy G tc (KJ/m 2 ) 1 3 rd mode Fracture energy G sc (KJ/m 2 ) 1 In addition, the throughthickness reinforcement in the stitched NCF composites is modeled in this section. Zhang et al. [47] and Liu et al. [48] first demonstrated an analytical model of zpin reinforced mode I and mode II delaminations. As shown in Fig.4.18 (a) and (b), DCB model was used to derive the bridging law of mode I delamination while threepoint bending model represented the mode II delamination 158
186 Chapter 4: Progressive Failure Analysis of NCF Composites bridging. Three typical pullout stages were discovered from both theoretical derivation and experiment [160]: 1. Elastic deformation with a full bonded interface. 2. Elastic deformation with a partially debonded interface. 3. Elastic deformation and frictional sliding with full debonded interface. Figure 4.18 Fiber pull out model [43]: (a) Mode I in DCB model; (b). Mode II in 3point bending model With the experimental verification, a trilinear loaddisplacement relationship was developed [160]. This method was further simplified to a bilinear constitutive model in the FE analysis to determine the mode I and II delamination toughness of zpinned laminates [43, 44]. Fig illustrates the schematic of the bilinear relationship, which 159
187 Chapter 4: Progressive Failure Analysis of NCF Composites is applied here to demonstrate the throughthickness reinforcement of stitches in NCF laminates: P stitch Pa stitch, 0 stitch a (4.27) a And Pa Pstitch Pa ( stitch a), a h (4.28) h a The above equations reveal that the pull out model is controlled by the peak bridging force P a and its corresponding displacement a. Before P a, the linear elastic behavior is defined according to the elastic tensile modulus of the stitches. When the pull out force excesses P a, the bridging force starts to reduce linearly until the ultimate pull out displacement h. In this study, the NCF plies are stitched by the polyester fibers. The material properties of the epoxy resin are thus used here for the polyester stitching fibers. The diameter of polyester fiber is 25 μm with filament number 40 according to vendor s specification. 160
188 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.19 Schematic of the bilinear relationship of the fiber bridging [43] The peak bridging P a is calculated as the axial force causes the shear off between the matrix and the stitching fibers. The equation can be expressed as, P N S A a s u s (4.29) Where S u denotes maximum shear strength and epoxy resin and stitches. A s is area of contact surface between the Ns is the filament number of stitches. Considering a stitching fiber embedding in the epoxy resin, the contact area is the laminate thickness h multiplies the perimeter of the stitching fiber, A s h d stitch (4.30) 161
189 Chapter 4: Progressive Failure Analysis of NCF Composites Furthermore, the displacement at peak load δ a can be written as, a hpa N A E s c stitch, (4.31) Where P a and A c is the crosssection area of single stitching fiber. As calculated, the values of a are N and mm, respectively. Note that the stitches are not explicitly modeled in this FE modeling. Instead, they are represented by the springs modeled along the thickness of the laminates. Similar modeling technique applied in [43] (also shown in Fig. 1.10) is deployed here. The interfacial nodes between adjacent layers, within the fiber bundle openings, are selected and paired with a springlike constraint. The spring elements are applied at the stitching locations between two stitched plies. The bilinear function described above is deployed here to describe the effective constitutive model of the nonlinear spring elements Simulation Results Uniaxial Tension is applied on both [0/90] 2s, [ 45] 2s NCF laminates (0 degree denotes the orientation along the loading direction). The stress contours 11 of these two laminates are presented in Fig and Fig Both of them clearly indicate that the stress concentrates in the vicinity of the stitches. In addition, the progressive damages are predicted for [0/90] 2s and [ 45] 2s NCF laminates (see Fig and 4.23). In both cases, the matrix damage in fiber yarns occurs earlier than the failure within the resin rich 162
190 Chapter 4: Progressive Failure Analysis of NCF Composites zones. Also, matrix failure initiates from the stitching sites that is coincident with predicted stress distributions. It is seen that, in [0/90] 2s laminates, more extensive matrix damages in 90 degree ply are obtained than in the 0 degree ply. Besides, the fiber failure is only found in the 0 degree ply and it follows the stitching patterns. The interlayer delaminations are also predicted in both biaxial laminates with an index between 0 (no delamination) and 1 (total delaminated). It is noted that the delamination in [0/90] 2s laminates does not play a vital role in the progressive failure behavior. The final delamination pattern is caused by the fiber fracture, which also coincides with the arrangement of stitches. On the other hand, there is no fiber breakage predicted prior to the final fracture of [ 45] 2s laminates, which is mainly attributed to the combination of intralayer matrix failure and interlayer delaminations (see Fig.4.23). 163
191 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.20 Local stress contours σ 11 of [0/90] 2s laminates under longitudinal tension BC1: (a). 0 ply; (b). 90 ply Figure 4.21 Local tress contours σ 11 in [ 45] 2s laminates under longitudinal tension BC1: (a). 45 ply; (b). +45 ply 164
192 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.22 Predicted progressive damages in [0/90] 2s laminates 165
193 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.23 Predicted progressive damages in [ 45] 2s laminates 166
194 Chapter 4: Progressive Failure Analysis of NCF Composites The simulations also predict the longitudinal stressstrain curves as shown in Fig The analysis reveals that the biaxial laminates are anisotropic materials as the modulus and strength in [0/90] 2s laminates (higher than 550MPa) exceed those in the [ 45] 2s laminates (less than150mpa). Besides, the stress strain relation in [0/90] 2s laminates is linear while there is high nonlinearity in the [ 45] 2s laminates. Here, to study the influence of the nonlinear modeling on the mechanical performance of the composites, the analysis based on the linear elastic material system is also conducted. As illustrated in Fig. 4.24, both linear and nonlinear models, present the similar shape of the stressstrain curve. In addition, in the [0/90] 2s composites, the linear modeling result is 2.48% higher than the nonlinear one, whereas in the [ 45] 2s laminates, the influence of the nonlinear modeling is more significant. The predicted longitudinal tensile strengths are listed in Table 4.8. It is seen that, in the [ 45] 2s laminates, the linear model predicts 24.57% higher tensile strength than the nonlinear model. This result suggests that the material nonlinearity of epoxy resin has stronger influence on the failure prediction when the laminates are subjected in inplane shear load ([ 45] 2s laminates) than the tensile load ([0/90] 2s laminates). This argument coincides with the study carried out by Vogler [27] and Pinho et al. [127]. The stressstrain curve also agrees well with Lomov et al. s [89] experimental data (see Fig. 4.1). 167
195 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.24 Longitudinal stressstrain curves from simulation results Table 4.8 Predicted longitudinal tensile strength Model Type Predicted Tensile Strength (MPa) Linear model of [0/90] 2s laminates Nonlinear model of [0/90] 2s laminates Linear model of [ 45] 2s laminates Nonlinear model of [ 45] 2s laminates Experimental Verification To verify the simulation results, four samples of [0/90] 2s laminates and five samples of [±45] 2s laminates are tested under a uniaxial tension. The experiment uses the same 168
196 Chapter 4: Progressive Failure Analysis of NCF Composites material system as in the numerical analysis. Epoxy is infused into the prelaid biaxial NCF fabrics with vacuum assisted resin transfer molding (VARTM). The specimens are cut from the composite panel by water jet cutting machine. The dimension of the sample is 200mm 24mm 2mm. As described in section 3.5, tensile test is conducted on an INSTRON 8501 machine at a constant displacement rate of 2mm/min. The experimental procedure follows the ASTM standard D3039. An extensometer is also used to measure the strain of the samples with the initial distance of 25mm. The tensile test results for both laminates are outlined in Table 4.9. The stressstrain curve is also validated through the experimental results. As shown in Fig. 4.25, for [0/90] 2s laminates, both linear and nonlinear analysis provide overestimations on tensile strength with deviations 10.2% and 7.5%, respectively. The mechanical response predicted from the analysis of [0/90] 2s laminates is consistent with the tensile test data. The damages observed in the specimens are also illustrated in Fig.4.26a. It presents the extensive matrix damages occurring in the 90 ply while Fig. 4.26b exhibits the fiber breakage at stitching sites of the 0 ply. The transverse matrix damage in the 0 ply (fiber splitting) is also observed from Fig. 4.26b. These damage patterns coincide with the predicted failure behavior presented in Fig Table 4.9 Experimental results of biaxial laminates Sample Ultimate tensile stress of [0/90] 2s (MPa) Ultimate tensile stress of [+/45] 2s (MPa) N.A. Mean value = Standard deviation =
197 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.25 Longitudinal stressstrain curves from simulation results Figure 4.26 Damage patterns of tested [0/90] 2s NCF specimens 170
198 Chapter 4: Progressive Failure Analysis of NCF Composites For [±45] 2s laminates, the mechanical nonlinearity can be clearly obtained from both experimental and numerical studies (see Fig. 4.27). It is seen that the nonlinear modeling effectively reduces the predicted tensile strength of [±45] 2s NCF composites. That is because the amplification method can capture the stress concentrations caused by the prefailure plastic yielding of matrix. In addition, the nonlinear modeling can predict the stressstrain relation which approaches more the experimental curves although the difference still exists to a certain extent. In previous section, it is exhibited that the final fracture of [ 45] 2s laminates is contributed by the combination of intralayer matrix failure and interlayer delaminations (see Fig. 4.23). This argument is verified by the damage patterns of tested sample shown in Fig. 4.28a where extensive matrix damages are observed at both +45 and 45 plies. In addition some delaminations are found at the edge of the specimens (shown in Fig. 4.28b) that agrees with the simulation result as well. Figure 4.27 Longitudinal stressstrain curves from simulation results 171
199 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.28 Damage patterns of tested [ 45] 2s NCF specimens 172
200 Chapter 4: Progressive Failure Analysis of NCF Composites 4.5 Macromechanics of NCF Composites Macroscopic Modeling In this section, the unnotched quasiisotropic [0/90/ 45] 2s (see Fig. 4.29) NCF laminates are studied based on the multiscale modeling across three length scales. The size of the FE model is 100mm 24mm x 2mm, and 3D 1 st order brick elements are used. The nonlinear material properties of the element in the macroscopic model are defined based on the mesoscale analysis of 0 ply as described in previous section. The stressstrain curves presented in Fig are fitted into the constitutive relations of global elements. Again, the tractionseparation law is applied to model the behavior of the nodes at the interply interface. Nonlinear spring elements are also applied to represent the stitching reinforcement. It is noted that the distributions of the spring elements should be coincident with the arrangement of stitching locations in actual specimens (see Fig. 4.30). With a quasistatic uniaxial tension applied (along the longitudinal direction x), the progressive failure analysis is implemented. 173
201 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.29 Layout of the quasiisotropic NCF laminates Figure 4.30 Arrangement of the spring element representing the throughthickness stitching 174
202 Chapter 4: Progressive Failure Analysis of NCF Composites Simulation Results The results of the progressive damage simulation are illustrated in Fig (a) through (e). Five stages in the development of damage are summarized as follows: a) The transverse matrix damage takes place first at both edges of the 90 ply (Fig. 4.31a. b) As shown in Fig b, matrix damage in the 90 ply propagates from the edges to the center of laminate. At longitudinal strain level 0.33%, delamination between 90 and 45 ply occurs. c) Subsequently, the damage evolutes to the matrix in both +45 and  45 plies. At the same time, delamination between +45 and  45 ply occurs at the edges (Fig c). d) Fig. 4.31d presents extensive matrix damages in all 90, +45 and  45 plies. Fiber failure initiates in 0 ply at the strain level 0.65%. e) The quasiisotropic laminate fails when the final fracture of fiber in 0 ply is exhibited. The ultimate tensile stress and failure strain are predicted (see Fig. 4.31e). 175
203 Chapter 4: Progressive Failure Analysis of NCF Composites The stressstrain curve is presented in Fig with the corresponding damage patterns. In summary, the 90 /45 interply is delaminated after the matrix failure in 90 ply. Thereafter, the matrix damage in +45 and  45 plies and the delamination between +45/ 45 ply take place. It revealed that when the quasiisotropic laminates are subjected to a uniaxial tension, the matrix damage in the transverse direction laminate (90 degree) takes place before the other failure modes. It is also reported that the quasiisotropic layout is susceptible to free edge delamination when loaded in uniaxial tension. To obtain a validation of the prediction, the tensile test on the quasiisotropic NCF laminates is conducted and presented in the next section. Figure 4.31(a). Predicted damages from macromechanical analysis at applied strain 0.18% 176
204 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.32(b). Predicted damages from macromechanical analysis at applied strain 0.33% 177
205 Chapter 4: Progressive Failure Analysis of NCF Composites 178
206 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.31(c). Predicted damages from macromechanical analysis at applied strain 0.38% 179
207 Chapter 4: Progressive Failure Analysis of NCF Composites 180
208 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.31(d). Predicted damages from macromechanical analysis at applied strain 0.65% 181
209 Chapter 4: Progressive Failure Analysis of NCF Composites 182
210 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.31(e). Predicted damages from macromechanical analysis at applied strain 1.29% 183
211 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.32 Predicted stressstrain relation from macromechanical analysis Experimental Verification In this section, uniaxial tensile test is performed on quasiisotropic NCF composite specimens. The experiment uses the same material system as in the numerical analysis and same procedure is conducted as in the validation test of biaxial laminates. The failure of tested specimen is shown in Fig All specimens have similar damage patterns. First, extensive matrix damages are observed in 90, +45 and  45 plies (see Fig. 4.33b), which agrees well with the simulation result. In addition, it shows that delaminations take place at the edge of the tested samples which appear at almost all the interfaces as shown in Fig. 4.33d. The numerical failure analysis provides similar delamination pattern between 90 /45 and +45/ 45 plies. But the extensive delamination at the interface 184
212 Chapter 4: Progressive Failure Analysis of NCF Composites between 0 /90 ply is not predicted by FE simulation and the reason is still not clear. The fiber fracture is also observed on the top 0 ply near the edge of the specimen (see Fig. 4.33c). Coincident fiber failure is predicted by simulation as shown in Fig. 4.33e. Predicted and experimental stressstrain relations are compared in Fig In the aspect of tensile strength, FE simulation can provide accurate ultimate tensile stress based on the proposed multiscale modeling method. The predicted ultimate strength is MPa that coincides with the average experimental data (434.7 ± 3.07 MPa). Fig also proves that the predicted progressive behaviors are coincident with the test results. Figure 4.33 Failure modes of tested quasiisotropic NCF specimens: (a) Top view for tested specimens; (b) Top view showing matrix damage; (c) Top view showing fiber fracture; (d) Section view showing delaminations 185
213 Chapter 4: Progressive Failure Analysis of NCF Composites Figure 4.34 Comparison of results between FE simulation and Experiment Sensitivity study is conducted for NCF composites and the results are outlined in Table Besides the geometric model and the fiber properties, the predicted performance of NCF composites greatly depends on the material nonlinearity of matrix and the fracture toughness values. Note that the mixmode fracture toughness for delamination significantly affect the tensile behavior of multiply NCF laminates while the throughthickness stitching has limited influence for the current material system. Unfortunately, reason of disparity between the simulation and experimental data for the progressive nonlinear behavior of [±45 ] laminates is still not clearly figured out. However, it is possible that the postfailure softening mode affects the accumulative damage behavior. In the current study, the linear softening model is consistently used. Thus a sensitivity study for the softening model to the textile composite failure analysis is recommended here. 186
214 Chapter 4: Progressive Failure Analysis of NCF Composites Table 4.10 Sensitivity study for NCF composites analysis Category Item Influenced object Sensitivity Geometric Modeling Resinrich zones for NCF composites Stress distribution Strain localization Damage initiations High Elastic Stiffness of fiber Longitudinal tensile behavior Dominantly Plasticity of matrix Shear and transverse behavior High Material Parameters Mode I Fiber fracture toughness Mixmode fracture toughness for delamination Ultimate tensile strength for longitudinal tension Ultimate tensile strength for inplane shear High High Throughthickness stitching N.A. Low Multiscale modeling techniques Postfailure softening mode Not clear Not clear 4.6 Conclusion In this chapter, the multiscale modeling method is extended to the progressive failure analysis of NCF composites, which has been developed with following new features: 1. A nonlinear multiscale modeling method is developed, which includes the elastoplastic constitutive modeling for epoxy resin and a novel nonlinear stress transfer method. 2. Nonlinear spring elements are applied to the FE model to represent the throughthickness stitching with prescribed stitching parameters. 187
215 Chapter 4: Progressive Failure Analysis of NCF Composites 3. Delamination is considered in both meso and macro failure analysis. The tractionseparation law is used to represent the constitutive behavior of cohesive interface. 4. The resinrich zones caused by the stitching needles are included in the mesomechanical models which is proven to be important because the stress distributions are strongly influenced by the resinrich zones. Two biaxial NCF laminates [0/90] 2s and [ 45] 2s are studied at meso level. The analysis results reveal that, in the case of [ 45] 2s laminates, the nonlinear modeling approach effectively reduces the predicted tensile strength and provides higher mechanical nonlinearity than the linear model. That is because the inplane tensile behavior of [ 45] 2s laminates are significantly influenced by the nonlinear properties of epoxy resin. In addition, it is not surprising that the [0/90] 2s laminates do not exhibit much influence of nonlinear modeling when they are under longitudinal tension. That is because the linear elastic fibers reinforcing along 0 degree sustain most of the tensile stresses. At the macro level, the mechanical response of unnotched quasiisotropic laminates is predicted and verified by experiment. As a result, the proposed method can precisely predict the damages and tensile performance. Extensive delaminations are observed in the tested specimen, which verifies the importance of delamination modeling in this failure analysis. 188
216 Chapter 5: Extension to Study of NCF Composites Containing Defects Chapter 5 Extension to Study of NCF Composites Containing Defects In this chapter, the multiscale modeling method is extended to the failure analysis of textile composites containing defects. The defects formed during the VARTM process for NCF composite laminates are studied here. Initially, section 5.1 presents the literature reviews of the studies for NCF composites containing the defects. Then, parametric study (no failure) is performed in section 5.2 to investigate the relations between the voids characteristics and the stiffness reductions. In section 5.3, defects are characterized into biaxial NCF laminates based on actual sample measurement, whereby progressive failure analysis can be performed to demonstrate the influence of the defects on the mechanical performance. Finally, simulation result is validated by the experiment in section Introduction to Defect Mechanics of Composite Materials The problem of defects can arise due to the heterogeneous nature of the composite materials. For textile composites, textile processing, composites manufacture, and handling can result in defects such as void (or porosity), matrix crack, fiber misalignment and delamination. Those common defects can affect the behavior of the composites. The influence of the defects on the mechanical performance of composites has been studied by numerous researchers. In term of the porosities, many studies [ ] reported that the fiberdominated mechanical properties were not significantly affected by the voids whilst the matrixdominated properties highly depended on their presence. 189
217 Chapter 5: Extension to Study of NCF Composites Containing Defects Generally, defect characterization is required to exam the quality of a composite structure in engineering applications. Conventional characterization techniques included density measurement [171], optical image analysis [171, 172] and the ultrasonic attenuation [173, 174]. Density measurement is based on Archimedes density theory. The ratio of actual sample density to the theoretical sample density can be calculated, based on weight and volume measurement, to determine the void volume fraction [171]. This method is quick and easy but strongly depends on the input properties of the fiber and matrix. Moreover, the optical image analysis based on the application of microscope has been widely used [172]. Its advantage is the visibility, which allows the identification of the void size, shape and distribution. Ultrasonic attenuation is another commonly used technique to determine the void level in the composites. The calibration curve can identify different void contents through presenting the variations in ultrasonic attenuation. This technique has been proven to be reliable and accurate [173, 174]. However, it is difficult to measure the void shape. Through the above techniques, the defects formed in the composite structures can be characterized. Several studies showed defects are dependent on the manufacturing process of composites. For instance, the voids in the composite laminates were compared between the material manufactured by resin transfer molding (RTM) and autoclave molding techniques [175, 176]. The differences were found with respect to defect location, shape, size, and volume fraction through microscope measurement and optical image analysis. Moreover, it is found that the defect characteristics also depend on the textile composite types. For example, Stone [177] reported the voids in UD laminates 190
218 Chapter 5: Extension to Study of NCF Composites Containing Defects tended to be small and spherical with small void content (<1.5%). Meanwhile, Hu et al. [178] presented the formation of voids in plain woven fabric composites was mainly located at the edge of transverse yarn (warp). Rubin and Jerina [179] also demonstrated that the voids in plain woven composites were truncated cone with a narrow elliptical cross section. It is believed that the shape of the void formed in the plain woven composites was related to the woven architecture and the yarn interactions For NCF composites, Lundstrom and Gebart [174] reported that, in the RTM manufactured NCF laminates, small long cylindrical bubbles formed inside the fiber bundles and larger spherical bubbles found in the space between the fiber bundles (see Fig. 5.1). Likewise, Schell et al. [180] demonstrated a multiscale defect system contained in textile composite laminates. The different air entrapped mechanisms explained the variation of defect formations. As illustrated in Fig. 5.2, when resin flowed into the fabrics, micro voids were created inside the fiber yarns at high injection pressure (Fig. 5.2a) while the mesoscale voids were created at low resininfusion velocity (Fig. 5.2b). 191
219 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.1 Multiscale defects observed in NCF composites [174] 192
220 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.2 Multiscale defects schematic in NCF composites [180] To study the defect behavior, defects mechanics were initially developed from Eshelby's inclusion theory [181]. Chao and Huang [181] presented an analytical method applying MoriTanaka s theory (based on inclusion Eshelby tensor) to predict the effective elastic stiffness of materials with various void contents and void aspect ratio. Madsen and Lilholt [182] developed a modified version of rule of mixtures to predict the tensile properties of composite materials. The effect of the composite void contents and anisotropy of fiber properties were also studied in his method. The numerical analysis method for defect modeling developed by Huang and Talreja [183] presented a computational scheme where the influence of defect shape on the elastic stiffness of unidirectional composite laminates was analyzed. In their work, the cigarshaped porosity was created with ellipticalcrosssection cylinder. Three defect 193
221 Chapter 5: Extension to Study of NCF Composites Containing Defects characteristics were studied: void content V v, length width ratio, and width height ratio. The parameters of the aspect ratios were determined from the average void length, width, and height from defect characterizations. The parametric study was carried out with void contents were chosen to vary from no void to 6%. In addition, the influences of varied void shape and size were also explored. The result revealed that the voids had much larger influence on reducing the matrixdominated properties than the fiberdominated one. In terms of the void shape, it was found that inplane properties were most sensitive to the widthheight ratio only. In addition flat voids had very limited effect on the outofplane properties and the long voids reduced the outofplane shear modulus. The numerical analysis result was also compared with the MoriTanaka method. As a result, FE model can present more accurate result than the analytical model through validation with experiment. 5.2 Study the Influence of Defects in NCF composites In this section, parametric study is first performed to investigate the effect of the defects on the elastic stiffness of NCF composites. A linear analysis is first carried out to study the stiffness reductions in the presence of mesoscale voids. A 3D RVE is then used to represent the 0 degree NCF laminate containing various defect characteristics. The quasistatic uniaixal tension is applied in this analysis. Later, meso failure analysis is performed through modeling mesoscale voids [174, 180] into the biaxial NCF composite laminates. Based on appropriate defect characterization, failure analysis of two biaxial NCF composites is performed to explore the influence of the mesoscale defects on the tensile 194
222 Chapter 5: Extension to Study of NCF Composites Containing Defects behavior. The defects are modeled into two mesoscale RVEs: [0/90] 2s and [±45] 2s laminates. The tensile test on the biaxial laminates is conducted to verify the analysis results Linear analysis The mesoscale model of 0 ply described in section is used here with same geometry and material properties. Parametric study is performed to investigate the influence of defects on the elastic inplane stiffness. The defect modeling strategy is presented in Fig Spherical voids are modeled as mesoscale defects in the center of the resinrich zones with various quantities and sizes. Corresponding void content V v can be obtained based on the simple calculations, V v nv v void 100% (5.1) V RVE Where n v denotes the number of voids. V void and V RVE indicate the volumes of the single void and the RVE, respectively. The finite element mesh of the laminate containing one 3D void is presented in Fig nd order tetrahedral elements (C3D10) are used with the range of element size from 0.01mm to 0.1mm. Finer mesh is seeded around the defect region. Same material properties are defined here as used for mesoscale analysis in Chapter
223 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.3 Defect modeling strategy in single NCF laminate Figure 5.4 Defect modeled in the FE model 196
224 Chapter 5: Extension to Study of NCF Composites Containing Defects The stress analysis of NCF laminate containing various defects is performed under three different inplane deformations ( xx, yy and xy ). It is noted that the analysis doesn t consider the damage. To illustrate the effect of voids, stress distributions in the laminate containing one void are enumerated in Fig. 5.5, which are compared with the stress contours of the laminate without any defect. Fig. 5.5 (b) and (c) exhibit that local transverse stress σ 22 and inplane shear stressτ 12 concentrate around the void when the laminate is under the transverse tension and inplane shear, respective. On the other hand, the distribution of longitudinal stress σ 11 is almost not affected by the defects (see Fig. 5.5 (a)). The stiffness reduction curves are also presented in Fig. 5.6 where the transverse modulus E 22 presents a most significant reduction (up to 5.3%) while the inplane shear modulus G 12 is reduced up to 3%. The longitudinal modulus E 11 exhibits the smallest reduction (less than 0.5%) due to the voids. The curves in Fig. 5.6 demonstrate linear correlations between void contents and the stiffness reductions. 197
225 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.5 Local stress contours in single NCF laminate: (a). Longitudinal stress 11 under BC1; (b). Transverse stress 22 under BC2; (c). Longitudinal inplane shear 12 under inplane shear BC4 Figure 5.6 Predicted inplane stiffness reductions with various void contents 198
226 Chapter 5: Extension to Study of NCF Composites Containing Defects Void content is not the only parameter studied in this section. Here, another series of linear analysis is performed to study the influence of void size and quantity on the inplane stiffness. Fig. 5.7 presents the defect modeling plan where the void content is kept constant at 0.6%, and the defect size and quantity varies (from three voids to eight voids). The result is illustrated in Fig. 5.8 that reveals relative small variation (< 0.5%) of stiffness reductions with respect to different void sizes and distributions. This analysis also proves that the void content is more significant in affecting the elastic stiffness of NCF laminate than the other parameters. Figure 5.7 Defect modeling strategy with fixed void content 0.6% 199
227 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.8 Predicted inplane stiffness reductions with fixed void contents Failure Analysis on Biaxial Laminates In this section, the defects in the biaxial NCF laminates are characterized based on actual specimen measurement. Then, progressive failure analysis is performed to study the influence of the defects on the tensile performance. Two RVE models representing two biaxial NCF laminates ([0/90] 2s and [±45] 2s ) are analyzed here. Finally, the simulation results are compared with the experimental data Defect Characterization The optical image analysis is applied here to identify the void size, shape and distribution of NCF composite laminates. Two types of biaxial NCF laminates [0/90] 2s and [ 45] 2s 200
228 Chapter 5: Extension to Study of NCF Composites Containing Defects are made by infusing the epoxy into the prelaid NCF fabrics with VARTM process. It is noted that 0 degree also denotes the direction of resin flow here. The rectangular composites samples are cut from the composite panels by water jet cutting machine. The dimensions of the composite samples are 24mm 24mm 2mm. To obtain high quality images from the microscope, the specimens are polished with gradually fine paper (320, 600, 800, 1200 grains/in). Totally 21 samples are measured with capturing 3 top images and 3 crosssection images from each one. Typical images are presented in Fig The mesosale voids defined in [180] are observed in both [0/90] 2s and [ 45] 2s laminates but with different defect characteristics. As illustrated in Fig. 5.9a, the voids within the resinrich zone of [0/90] 2s laminates present spherical shape. The range of void diameters is from 0.097mm to 0.187mm with an average value of 0.14mm ( 0.043). Based on that, the average void volume fraction can be calculated as 0.032%. It is noted that this volume fraction takes account of the mesoscale voids only. The micro voids inside the fiber yarn are not included in this study. Moreover, the voids in [ 45] 2s laminates are characterized in Fig. 5.9b. Unlike in [0/90] 2s laminates, the voids in [ 45] 2s laminates present ellipsoidal shape. Normally, two voids are observed in each resinrich zone and the shape aligns with the contour of the resin eyes. It is measured that the range of void major axis length is from 0.33mm to 1.23mm. The mean axis lengths of those 3D ellipsoidal voids are 0.82mm ( 0.27), 0.32mm ( 0.089), and 0.28mm ( 0.067). Correspondingly, the average void content is about 4.4%, which is much higher than the void content in [0/90] 2s laminates. The reason behind this difference is explained here (see Fig. 5.10). Given that the resininfusion flow direction is along 0 degree, it provides higher infusion velocity in [0/90] 2s laminates than in [ 45] 2s laminates. Smaller voids are 201
229 Chapter 5: Extension to Study of NCF Composites Containing Defects thus created in the [0/90] 2s laminates. In a word, the defect characteristics in NCF are influenced by the resininfusion direction, fiber yarn orientation, and geometry of the resin eyes. Fig. 5.9 (a) Defects observed in [0/90] 2s laminates Fig. 5.9 (b) Defects observed in [ 45] 2s laminates 202
230 Chapter 5: Extension to Study of NCF Composites Containing Defects Fig Defects schematic for biaxial NCF composites: (a) defect in [0/90] 2s laminates; (b) defect in [ 45] 2s laminates Case [0/90] 2s Laminates Based on the above defect characterization, spherical voids with varied sizes are modeled at each resinrich zone in [0/90] 2s laminates (see Fig. 5.11). Uniaxial tension is applied along the fiber direction in 0 ply. Typical progressive damages are illustrated in Fig (when V v is 0.032%). A good comparison can be obtained between Fig and Fig , which reveals that the presence of defects has very limited effect on the damage behavior of [0/90] 2s laminates. In addition, the simulation results are outlined in Table 5.1, which lists the predicted tensile modulus and ultimate tensile strength with different void contents. It is not surprising that the reductions of both tensile stiffness and tensile strength are very small due to very low void content. 203
231 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.11 Defect modeling strategy in [0/90] 2s NCF laminates 204
232 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.12 Progressive damages in [0/90] 2s NCF laminates Table 5.1 Simulation results of [0/90] 2s laminates containing mesoscale defects Vv Tensile Modulus (GPa) Reduction of Tensile Modulus Ultimate Tensile Strength (MPa) Reduction of Ultimate Tensile Strength 0.000% % % 0.011% % % 0.020% % % 0.032% % % 0.076% % % 205
233 Chapter 5: Extension to Study of NCF Composites Containing Defects To validate the prediction result, the results of tensile test conducted for [0/90] 2s laminates (see section 4.4.3) are compared here. The stressstrain curves of both experimental and predicted results presented in Fig Again, it demonstrates that the effect of the mesoscale void is insignificant in [0/90] 2s laminates. Figure 5.13 Predicted stressstrain curve from FE simulation of [0/90] 2s NCF laminates 206
234 Chapter 5: Extension to Study of NCF Composites Containing Defects Case [±45] 2s Laminates As discussed in previous sections, the ellipsoidal defects formed in [±45] 2s laminates have a much higher volume content than in [0/90] 2s laminates. Fig illustrates the defect modeling plan, where duovoid is modeled in each resinrich zone with five different sizes. Here, the lengths of major axis of the ellipsoidal defects are varied while the minor axis length remains constant. Based on that, the progressive failure analysis is performed with a uniaxial tension along 0 degree. The damage patterns at applied strain level ε xx = 1.3% for different void contents are presented in Fig It exhibits that, when the voids become larger, more matrix damages concentrate around the defects rather than propagate to the fiber yarns. Table 5.2 lists the predicted tensile modulus and ultimate tensile strength with various void contents in [±45] 2s laminates. With a void content range between 1.75% and 6.59%, maximum reductions of 11.16% and 8.06% are predicted for tensile modulus and tensile strength, respectively. 207
235 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.14 Defect modeling strategy in [±45] 2s NCF laminates 208
236 Chapter 5: Extension to Study of NCF Composites Containing Defects Figure 5.15 Progressive damages in [±45] 2s NCF laminates at different applied strain levels Table 5.2 Simulation results of [±45] 2s laminates containing mesoscale defects V v Tensile Modulus (GPa) Reduction of Tensile Modulus Ultimate Tensile Strength (MPa) Reduction of Ultimate Tensile Strength 0.00% % % 1.75% % % 3.22% % % 4.40% % % 5.36% % % 6.59% % % To validate the simulation results, the test results for five [±45] 2s laminates samples are compared here (see section 4.4.3). The predicted stressstrain curves are validated by the 209
EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationAlternative numerical method in continuum mechanics COMPUTATIONAL MULTISCALE. University of Liège Aerospace & Mechanical Engineering
University of Liège Aerospace & Mechanical Engineering Alternative numerical method in continuum mechanics COMPUTATIONAL MULTISCALE Van Dung NGUYEN Innocent NIYONZIMA Aerospace & Mechanical engineering
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More information2 Experiment of GFRP bolt
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FATIGUE LIFE EVALUATION OF BOLT MADE OF WOVEN FABRIC FRP Takeshi INOUE*, Hiroaki NAKAI**, Tetsusei KURASHIKI**, Masaru ZAKO**, Yuji KOMETANI*** *Graduate
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationEffects of mesostructure on the inplane properties of tufted carbon fabric composites
Effects of mesostructure on the inplane properties of tufted carbon fabric composites CompTest 2011, 14 th February 2011 Johannes W G Treiber Denis D R Cartié Ivana K Partridge j.treiber@cranfield.ac.uk
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationComposites Science and Technology
Composites Science and Technology 7 (1) 194 1941 Contents lists available at ScienceDirect Composites Science and Technology journal homepage: www.elsevier.com/locate/compscitech Local damage in a 5harness
More informationENGN 2340 Final Project Report. Optimization of Mechanical Isotropy of Soft Network Material
ENGN 2340 Final Project Report Optimization of Mechanical Isotropy of Soft Network Material Enrui Zhang 12/15/2017 1. Introduction of the Problem This project deals with the stressstrain response of a
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationTable of Contents. Preface...xvii. Part 1. Level
Preface...xvii Part 1. Level 1... 1 Chapter 1. The Basics of Linear Elastic Behavior... 3 1.1. Cohesion forces... 4 1.2. The notion of stress... 6 1.2.1. Definition... 6 1.2.2. Graphical representation...
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationMicrostructural Randomness and Scaling in Mechanics of Materials. Martin OstojaStarzewski. University of Illinois at UrbanaChampaign
Microstructural Randomness and Scaling in Mechanics of Materials Martin OstojaStarzewski University of Illinois at UrbanaChampaign Contents Preface ix 1. Randomness versus determinism ix 2. Randomness
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationModelling of Spread Tow Carbon Fabric Composites for Advanced Lightweight Products EMINA MUSIC ANDREAS WIDROTH. Master s thesis in Applied Mechanics
Modelling of Spread Tow Carbon Fabric Composites for Advanced Lightweight Products Master s thesis in Applied Mechanics EMINA MUSIC ANDREAS WIDROTH Department of Applied Mechanics Division of Material
More informationTABLE OF CONTENTS CHAPTER TITLE PAGE DECLARATION DEDICATION ACKNOWLEDGEMENT ABSTRACT ABSTRAK
vii TABLE OF CONTENTS CHAPTER TITLE PAGE DECLARATION DEDICATION ACKNOWLEDGEMENT ABSTRACT ABSTRAK TABLE OF CONTENTS LIST OF TABLES LIST OF FIGURES LIST OF ABBREVIATIONS LIST OF SYMBOLS ii iii iv v vi vii
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationAn overview of Carbon Fiber modeling in LSDYNA. John Zhao October 23 th 2017
An overview of Carbon Fiber modeling in LSDYNA John Zhao zhao@lstc.com October 23 th 2017 Outline Manufacturing of Carbon Fiber Compression molding *MAT_277 & 278 *MAT_293 *MAT_249 Resin transform molding
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationPowerful Modelling Techniques in Abaqus to Simulate
Powerful Modelling Techniques in Abaqus to Simulate Necking and Delamination of Laminated Composites D. F. Zhang, K.M. Mao, Md. S. Islam, E. Andreasson, Nasir Mehmood, S. KaoWalter Email: sharon.kaowalter@bth.se
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationDevelopment of a Progressive Failure Model for Notched Woven Composite Laminates. Daniel Christopher Munden
Development of a Progressive Failure Model for Notched Woven Composite Laminates Daniel Christopher Munden Thesis submitted to the faculty of the Virginia Polytechnic Institute and State University in
More informationPREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL BRAIDED COMPOSITES USING BEAM UNIT CELLS
THE 19TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL 1 J. Cichosz1*, J. Bückle1, R. Hinterhölzl1, M. Wolfahrt2 Institute for Carbon Composites, Technische
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationCrashworthiness of Composite Structures with Various Fiber Architectures
11 th International LDYNA Users Conference Crash afety Crashworthiness of Composite tructures with Various Fiber Architectures Nageswara R. Janapala 1, FuKuo Chang, Robert K. Goldberg 3, Gary D. Roberts
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationDiscrete Element Modelling of a Reinforced Concrete Structure
Discrete Element Modelling of a Reinforced Concrete Structure S. Hentz, L. Daudeville, F.V. Donzé Laboratoire Sols, Solides, Structures, Domaine Universitaire, BP 38041 Grenoble Cedex 9 France sebastian.hentz@inpg.fr
More informationNumerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions
Numerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions Numerical Analysis of Delamination Behavior in Laminated Composite with
More informationANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS ANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES Deepak Goyal*, John D. Whitcomb*, Julian Varghese* *Department of Aerospace Engineering,
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationDepartment of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India
Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationEsben Byskov. Elementary Continuum. Mechanics for Everyone. With Applications to Structural Mechanics. Springer
Esben Byskov Elementary Continuum Mechanics for Everyone With Applications to Structural Mechanics Springer Contents Preface v Contents ix Introduction What Is Continuum Mechanics? "I Need Continuum Mechanics
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationComparison between a Cohesive Zone Model and a Continuum Damage Model in Predicting ModeI Fracture Behavior of Adhesively Bonded Joints
Copyright 2012 Tech Science Press CMES, vol.83, no.2, pp.169181, 2012 Comparison between a Cohesive Zone Model and a Continuum Damage Model in Predicting ModeI Fracture Behavior of Adhesively Bonded
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationMICROMECHANICAL ANALYSIS OF WOVEN COMPOSITES USING VARIATIONAL ASYMPTOTIC METHOD
MICROMECHANICAL ANALYSIS OF WOVEN COMPOSITES USING VARIATIONAL ASYMPTOTIC METHOD Rajeev G. Nair 1,2, B. Sivasubramonian 2, P. J. Guruprasad 1 1 Department of Aerospace Engineering, Indian Institute of
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFinal Analysis Report MIE 313 Design of Mechanical Components
Final Analysis Report MIE 313 Design of Mechanical Components Juliana Amado Charlene Nestor Peter Walsh Table of Contents Abstract:...iii Introduction:... 4 Procedure:... 5 Results:... 6 Reliability:...
More informationEDEM DISCRETIZATION (Phase II) Normal Direction Structure Idealization Tangential Direction Pore spring Contact spring SPRING TYPES Inner edge Inner d
Institute of Industrial Science, University of Tokyo Bulletin of ERS, No. 48 (5) A TWOPHASE SIMPLIFIED COLLAPSE ANALYSIS OF RC BUILDINGS PHASE : SPRING NETWORK PHASE Shanthanu RAJASEKHARAN, Muneyoshi
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationOverview of Probabilistic Modeling of Woven Ceramic Matrix Composites ABSTRACT
ABSTRACT An overview of current research efforts in understanding the cause of variability in the thermomechanical properties of woven ceramic matrix composites is presented. Statistical data describing
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationTHERMOELASTIC PROPERTIES PREDICTION OF 3D TEXTILE COMPOSITES
THERMOELASTI PROPERTIES PREDITION OF 3D TEXTILE OMPOSITES S. P. Yushanov, A. E. Bogdanovich, and M. H. Mohamed 3TEX, Inc., 117 Main ampus Drive, Suite 32, Raleigh, N 2766, U.S.A. SUMMARY: Predictive methodology
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationMicromechanics Based Multiscale Modeling. of the Inelastic Response and Failure of. Complex Architecture Composites. Kuang Liu
Micromechanics Based Multiscale Modeling of the Inelastic Response and Failure of Complex Architecture Composites by Kuang Liu A Dissertation Presented in Partial Fulfillment of the Requirements for the
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationMesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method
Mesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method J. Xu a*, SV. Lomov a, I. Verpoest a, S. Daggumati b, W. Van Paepegem b, J. Degrieck b a Katholieke
More informationNonlinearities in mechanical behavior of textile composites
Composite Structures 71 (25) 61 67 www.elsevier.com/locate/compstruct Nonlinearities in mechanical behavior of textile composites Enrico DÕAmato Energetics Departement, L Aquila University, 674 Monteluco
More informationSlow Velocity Flow Fields in Composite Materials
Slow Velocity Flow Fields in Composite Materials A Coupled Problem by the Homogenization Method Noboru Kikuchi and His Associates The University of Michigan Ann Arbor, MI 48109, USA Major Contributors
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationA FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES
ECCM6 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 24 A FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES J. Främby, J. Brouzoulis,
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationCrashworthiness of composite structures: Experiment and Simulation
Crashworthiness of composite structures: Experiment and Simulation Francesco Deleo, Bonnie Wade and Prof. Paolo Feraboli (UW) Dr. Mostafa Rassaian (Boeing R&T) JAMS 2010 The Joint Advanced Materials and
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More information